# Supplementary Information (SI) for Materials Chemistry Frontiers.
# This journal is © the Partner Organisations 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ee109_forrevisions
_database_code_depnum_ccdc_archive 'CCDC 2371927'
loop_
_audit_author_name
_audit_author_address
'Eslam M. Elbakry'
;The University of Alabama
United States of America
;
_audit_update_record             
;
2024-09-24 deposited with the CCDC.	2024-10-16 downloaded from the CCDC.
;
# start Validation Reply Form
_vrf_PLAT097_ee109_forrevisions  
;
PROBLEM: Large Reported Max.  (Positive) Residual Density       8.02 eA-3
RESPONSE: Residual peak accounts for 5% of A-site electron density. The residual is interpreted as arising from local structure correlations that cannot be modeled physically in the current unit cell. The residual was used to determine total occupancy of the channels but is not included in the model so as to avoid misleading cation geometry
;
_vrf_PLAT112_ee109_forrevisions  
;
PROBLEM: ADDSYM Detects New (Pseudo) Symm. Elem        -4        100 %Fit
RESPONSE: ADDSYM excludes the disordered sites that break the pseudosymmetry. Lattice system is unambiguously monoclinic.
;
_vrf_PLAT113_ee109_forrevisions  
;
PROBLEM: ADDSYM Suggests Possible Pseudo/New  Space Group       P4/n Check
RESPONSE: ADDSYM excludes the disordered sites that break the pseudosymmetry. Lattice system is unambiguously monoclinic.
;
_vrf_PLAT042_ee109_forrevisions  
;
PROBLEM: Calc. and Reported MoietyFormula Strings  Differ     Please Check
RESPONSE: The difference is accounted for in the maximum residual peak.
;
# Added during the CSD deposition process: Tuesday 24 September 2024 05:49 PM
# end Validation Reply Form

_audit_creation_date             2024-09-03
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6408)
;
_shelx_SHELXL_version_number     2014/7
loop_
_audit_author_email
jmallred@ua.edu
emelbakry@crimson.ua.edu
_chemical_name_common            Na1/3BaMo8O16
_chemical_name_systematic        ?
_chemical_formula_moiety         'Ba0.943 Mo8 Na0.306 O16'
_chemical_formula_sum            'Ba0.94 Mo8 Na0.31 O16'
_chemical_formula_weight         1160.32
_chemical_melting_point          ?
_chemical_oxdiff_formula         'Na0.325 Ba1.006 Mo8 O16'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_H-M_alt        'P 1 2/n 1'
_space_group_name_Hall           '-P 2yac'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y, -z+1/2'
'-x, -y, -z'
'x-1/2, -y, z-1/2'

_cell_length_a                   10.22775(19)
_cell_length_b                   5.73224(12)
_cell_length_c                   10.2849(2)
_cell_angle_alpha                90
_cell_angle_beta                 90.2821(18)
_cell_angle_gamma                90
_cell_volume                     602.98(2)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    10205
_cell_measurement_temperature    299.4(6)
_cell_measurement_theta_max      43.0460
_cell_measurement_theta_min      2.7880
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    11.169
_exptl_absorpt_correction_T_max  0.750
_exptl_absorpt_correction_T_min  0.589
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.40.16b (Rigaku Oxford Diffraction, 2018)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    6.391
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             1041
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
2 1 -1 0.0360
-2 1 1 0.0331
2 -1 -1 0.0289
-2 -1 1 0.0057
1 2 -2 0.0474
-1 -2 2 0.0127
2 0 -1 0.0393
2 0 1 0.0080
-2 0 -1 0.0241
0 1 2 0.0161
0 -1 -2 0.0323
0 0 1 0.0115
0 0 -1 0.0535

_exptl_crystal_size_max          0.063
_exptl_crystal_size_mid          0.059
_exptl_crystal_size_min          0.032
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
1.9897 1.0018 -1.0138 0.0483 0.1920 0.0063
-1.9967 0.9979 1.0144 -0.0968 -0.0148 -0.1722
1.9967 -0.9979 -1.0144 0.0968 0.0148 0.1722
-1.9897 -1.0018 1.0138 -0.0483 -0.1920 -0.0063
0.9800 2.0007 -2.0053 0.0890 0.2407 -0.1382
-0.9800 -2.0007 2.0053 -0.0890 -0.2407 0.1382
1.9932 0.0019 -1.0141 0.0725 0.1034 0.0892
2.0060 0.0019 0.9843 -0.0624 0.0875 0.1118
-2.0060 -0.0019 -0.9843 0.0624 -0.0875 -0.1118
0.0093 0.9999 1.9987 -0.1592 0.0728 -0.0604
-0.0093 -0.9999 -1.9987 0.1592 -0.0728 0.0604
0.0064 -0.0000 0.9992 -0.0675 -0.0079 0.0113
-0.0064 0.0000 -0.9992 0.0675 0.0079 -0.0113

_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0247
_diffrn_reflns_av_unetI/netI     0.0260
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.974
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            15889
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.974
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         42.980
_diffrn_reflns_theta_min         1.980
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      299.4(6)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean ?
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measurement_details      
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω     58.00  84.00   0.50   10.00    --   37.19 159.00-159.00   52
  2  ω    -10.00  16.00   0.50   10.00    --   37.19 -57.00-164.00   52
  3  ω     57.00  82.00   0.50   10.00    --   37.19 178.00   0.00   50
  4  ω    -37.00  21.00   0.50   10.00    --   37.19 -28.00 170.63  116
  5  ω    -34.00  26.00   0.50   10.00    --   37.19 -43.00  93.32  120
  6  ω    -23.00   2.00   0.50   10.00    --   37.19 -19.00-120.00   50
  7  ω      1.00  66.00   0.50   10.00    --   37.19 -99.00  30.00  130
  8  ω      2.00  28.00   0.50   10.00    --   37.19 -19.00 -90.00   52
  9  ω     27.00  68.00   0.50   10.00    --   37.19  44.00  40.23   82
 10  ω     64.00  90.00   0.50   10.00    --   37.19  37.00 -60.00   52
 11  ω     77.00 106.00   0.50   10.00    --   37.19  37.00  60.00   58
 12  ω     44.00 100.00   0.50   10.00    --   37.19  57.00  90.00  112
 13  ω     34.00  59.00   0.50   10.00    --   37.19  37.00  30.00   50
 14  ω    -16.00   9.00   0.50   10.00    --   37.19 -19.00-150.00   50
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type       
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0020445000
_diffrn_orient_matrix_UB_12      -0.0242217000
_diffrn_orient_matrix_UB_13      -0.0675659000
_diffrn_orient_matrix_UB_21      0.0475901000
_diffrn_orient_matrix_UB_22      0.0887653000
_diffrn_orient_matrix_UB_23      -0.0082204000
_diffrn_orient_matrix_UB_31      0.0504191000
_diffrn_orient_matrix_UB_32      -0.0827750000
_diffrn_orient_matrix_UB_33      0.0109601000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Rotating-anode X-ray tube'
_diffrn_source_type              'Rigaku (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                3854
_reflns_number_total             4294
_reflns_odcompleteness_completeness 99.56
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'CrysAlisPro 1.171.40.16b (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.40.16b (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.40.16b (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2014/7 (Sheldrick, 2015)'
_computing_structure_solution    ?
_refine_diff_density_max         8.019
_refine_diff_density_min         -1.977
_refine_diff_density_rms         0.351
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.062
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     126
_refine_ls_number_reflns         4294
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0286
_refine_ls_R_factor_gt           0.0245
_refine_ls_restrained_S_all      1.062
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0289P)²+2.4972P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0620
_refine_ls_wR_factor_ref         0.0634
_refine_special_details          'Refined as a 2-component twin.,Twin'
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.9953(7)
 0.0047(7)
2. Shared sites
{Na1A, Ba1A}
{Na1B, Ba1B}
{Na2A, Ba2A}
{Na2B, Ba2B}
3. Uiso/Uaniso restraints and constraints
Uanis(Na1A) = Uanis(Ba1A) = Uanis(Na2A) = Uanis(Ba2A)
Uanis(Na1B) = Uanis(Ba1B) = Uanis(Na2B) = Uanis(Ba2B)
4. Others
 Sof(Na1A)=0.1224*FVAR(2)
 Sof(Ba1A)=0.3776*FVAR(2)
 Sof(Na2A)=0.1224*FVAR(3)
 Sof(Ba2A)=0.3776*FVAR(3)
 Sof(Na2B)=0.1224*FVAR(4)
 Sof(Ba2B)=0.3776*FVAR(4)
 Sof(Na1B)=0.1224*FVAR(5)
 Sof(Ba1B)=0.3776*FVAR(5)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1A Ba 0.2500 -0.0430(9) 0.7500 0.0059(4) Uani 0.146(12) 2 d S T P A 1
Na1A Na 0.2500 -0.0430(9) 0.7500 0.0059(4) Uani 0.047(4) 2 d S T P A 1
Ba1B Ba 0.2500 -0.0955(14) 0.7500 0.0150(5) Uani 0.381(13) 2 d S T P A 2
Na1B Na 0.2500 -0.0955(14) 0.7500 0.0150(5) Uani 0.124(4) 2 d S T P A 2
Ba2A Ba 0.2500 0.2721(8) 0.7500 0.0059(4) Uani 0.185(11) 2 d S T P A 3
Na2A Na 0.2500 0.2721(8) 0.7500 0.0059(4) Uani 0.060(4) 2 d S T P A 3
Ba2B Ba 0.2500 0.3239(18) 0.7500 0.0150(5) Uani 0.231(11) 2 d S T P A 4
Na2B Na 0.2500 0.3239(18) 0.7500 0.0150(5) Uani 0.075(3) 2 d S T P A 4
Mo1 Mo 0.43134(2) 0.61618(3) 0.42042(2) 0.00277(3) Uani 1 1 d . . . . .
Mo2 Mo 0.42496(2) 0.16683(3) 0.40104(2) 0.00332(3) Uani 1 1 d . . . . .
Mo3 Mo 0.41723(2) 0.40093(3) 0.07320(2) 0.00317(3) Uani 1 1 d . . . . .
Mo4 Mo 0.39595(2) 0.84549(3) 0.08001(2) 0.00349(3) Uani 1 1 d . . . . .
O1 O 0.41767(16) 0.6064(3) 0.61926(17) 0.0051(2) Uani 1 1 d . . . . .
O2 O 0.44024(16) 0.1098(3) 0.59622(16) 0.0045(2) Uani 1 1 d . . . . .
O3 O 0.41906(17) 0.6272(3) 0.22081(16) 0.0054(2) Uani 1 1 d . . . . .
O4 O 0.41867(17) 0.1244(3) 0.20812(16) 0.0054(2) Uani 1 1 d . . . . .
O5 O 0.61745(17) 0.3767(3) 0.07986(16) 0.0054(2) Uani 1 1 d . . . . .
O6 O 0.59344(16) 0.8777(3) 0.05329(16) 0.0048(2) Uani 1 1 d . . . . .
O7 O 0.28124(16) 0.3839(3) 0.41589(17) 0.0050(2) Uani 1 1 d . . . . .
O8 O 0.21132(16) 0.8831(3) 0.08279(17) 0.0052(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1A Mo2 3.7443(10) 4_556 ?
Ba1A Mo2 3.7443(10) 3_656 ?
Ba1A Mo4 3.7560(9) 1_546 ?
Ba1A Mo4 3.7560(9) 2_545 ?
Ba1A O1 2.968(4) 2_546 ?
Ba1A O1 2.968(4) 1_545 ?
Ba1A O2 2.662(2) . ?
Ba1A O2 2.662(2) 2_556 ?
Ba1A O5 2.922(4) 3_656 ?
Ba1A O5 2.922(4) 4_556 ?
Ba1A O6 2.743(3) 4_566 ?
Ba1A O6 2.743(3) 3_666 ?
Ba1B Mo2 3.6991(9) 4_556 ?
Ba1B Mo2 3.6991(9) 3_656 ?
Ba1B Mo4 3.7166(7) 1_546 ?
Ba1B Mo4 3.7166(7) 2_545 ?
Ba1B O1 2.773(5) 2_546 ?
Ba1B O1 2.773(5) 1_545 ?
Ba1B O2 2.775(4) . ?
Ba1B O2 2.775(4) 2_556 ?
Ba1B O5 2.734(5) 3_656 ?
Ba1B O5 2.734(5) 4_556 ?
Ba1B O6 2.861(4) 4_566 ?
Ba1B O6 2.861(4) 3_666 ?
Ba2A Mo1 3.7630(8) 3_666 ?
Ba2A Mo1 3.7630(8) 4_566 ?
Ba2A Mo3 3.8031(9) 2 ?
Ba2A Mo3 3.8031(9) 1_556 ?
Ba2A O1 2.906(3) . ?
Ba2A O1 2.906(3) 2_556 ?
Ba2A O2 2.680(2) . ?
Ba2A O2 2.680(2) 2_556 ?
Ba2A O5 2.988(4) 3_666 ?
Ba2A O5 2.988(4) 4_566 ?
Ba2A O6 2.713(2) 4_566 ?
Ba2A O6 2.713(2) 3_666 ?
Ba2B Mo1 3.7240(10) 4_566 ?
Ba2B Mo1 3.7240(10) 3_666 ?
Ba2B Mo3 3.7568(13) 2 ?
Ba2B Mo3 3.7568(13) 1_556 ?
Ba2B O1 2.719(7) . ?
Ba2B O1 2.719(7) 2_556 ?
Ba2B O2 2.797(5) . ?
Ba2B O2 2.797(5) 2_556 ?
Ba2B O5 2.797(7) 4_566 ?
Ba2B O5 2.797(7) 3_666 ?
Ba2B O6 2.821(5) 3_666 ?
Ba2B O6 2.821(5) 4_566 ?
Mo1 Ba2A 3.7630(8) 3_666 ?
Mo1 Ba2B 3.7240(10) 3_666 ?
Mo1 Mo1 2.5305(4) 3_666 ?
Mo1 Mo2 2.5842(3) . ?
Mo1 Mo2 3.1634(3) 1_565 ?
Mo1 Mo2 2.6556(3) 3_666 ?
Mo1 O1 2.0458(16) 3_666 ?
Mo1 O1 2.0512(17) . ?
Mo1 O2 2.0554(16) 3_666 ?
Mo1 O3 2.0572(17) . ?
Mo1 O7 2.0324(16) . ?
Mo1 O8 2.1142(16) 2 ?
Mo2 Ba1B 3.6990(9) 3_656 ?
Mo2 Na1B 3.6990(9) 3_656 ?
Mo2 Mo1 2.6556(3) 3_666 ?
Mo2 Mo1 3.1634(3) 1_545 ?
Mo2 Mo2 3.1823(4) 3_656 ?
Mo2 O1 2.0801(17) 3_666 ?
Mo2 O2 2.1012(16) 3_656 ?
Mo2 O2 2.0391(17) . ?
Mo2 O4 1.9998(17) . ?
Mo2 O7 1.9327(16) . ?
Mo2 O8 2.1492(16) 2_545 ?
Mo3 Ba2A 3.8031(9) 1_554 ?
Mo3 Ba2B 3.7568(13) 1_554 ?
Mo3 Mo3 2.5394(3) 3_665 ?
Mo3 Mo4 2.8564(3) 3_665 ?
Mo3 Mo4 3.1921(3) 1_545 ?
Mo3 Mo4 2.5586(3) . ?
Mo3 O3 1.9970(17) . ?
Mo3 O4 2.1069(17) . ?
Mo3 O5 2.0548(17) 3_665 ?
Mo3 O5 2.0533(17) . ?
Mo3 O6 2.0624(16) 3_665 ?
Mo3 O7 2.0358(16) 2 ?
Mo4 Ba1A 3.7560(9) 1_564 ?
Mo4 Ba1B 3.7166(8) 1_564 ?
Mo4 Na1B 3.7166(8) 1_564 ?
Mo4 Mo3 2.8564(3) 3_665 ?
Mo4 Mo3 3.1921(3) 1_565 ?
Mo4 O3 1.9273(16) . ?
Mo4 O4 2.0838(17) 1_565 ?
Mo4 O5 2.0839(17) 3_665 ?
Mo4 O6 2.0482(16) . ?
Mo4 O6 2.1002(16) 3_675 ?
Mo4 O8 1.9009(16) . ?
O1 Ba1A 2.968(4) 1_565 ?
O1 Na1A 2.968(4) 1_565 ?
O1 Ba1B 2.773(5) 1_565 ?
O1 Na1B 2.773(5) 1_565 ?
O1 Mo1 2.0458(16) 3_666 ?
O1 Mo2 2.0801(17) 3_666 ?
O2 Mo1 2.0554(16) 3_666 ?
O2 Mo2 2.1012(16) 3_656 ?
O4 Mo4 2.0839(17) 1_545 ?
O5 Ba1A 2.922(4) 3_656 ?
O5 Na1A 2.922(4) 3_656 ?
O5 Ba1B 2.734(5) 3_656 ?
O5 Na1B 2.734(5) 3_656 ?
O5 Ba2A 2.988(4) 3_666 ?
O5 Na2A 2.988(4) 3_666 ?
O5 Ba2B 2.797(7) 3_666 ?
O5 Na2B 2.797(7) 3_666 ?
O5 Mo3 2.0548(17) 3_665 ?
O5 Mo4 2.0840(17) 3_665 ?
O6 Ba1A 2.743(3) 3_666 ?
O6 Na1A 2.743(3) 3_666 ?
O6 Ba1B 2.861(4) 3_666 ?
O6 Na1B 2.861(4) 3_666 ?
O6 Ba2A 2.713(2) 3_666 ?
O6 Na2A 2.713(2) 3_666 ?
O6 Ba2B 2.821(5) 3_666 ?
O6 Na2B 2.821(5) 3_666 ?
O6 Mo3 2.0624(16) 3_665 ?
O6 Mo4 2.1002(16) 3_675 ?
O7 Mo3 2.0358(16) 2 ?
O8 Mo1 2.1143(16) 2 ?
O8 Mo2 2.1491(16) 2_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo2 Ba1A Mo2 158.14(16) 4_556 3_656 ?
Mo2 Ba1A Mo4 86.71(3) 3_656 2_545 ?
Mo2 Ba1A Mo4 86.71(3) 4_556 1_546 ?
Mo2 Ba1A Mo4 89.59(3) 4_556 2_545 ?
Mo2 Ba1A Mo4 89.59(3) 3_656 1_546 ?
Mo4 Ba1A Mo4 160.40(16) 2_545 1_546 ?
O1 Ba1A Mo2 33.65(3) 2_546 4_556 ?
O1 Ba1A Mo2 125.15(16) 1_545 4_556 ?
O1 Ba1A Mo2 125.15(16) 2_546 3_656 ?
O1 Ba1A Mo2 33.65(3) 1_545 3_656 ?
O1 Ba1A Mo4 93.80(9) 2_546 2_545 ?
O1 Ba1A Mo4 72.74(6) 2_546 1_546 ?
O1 Ba1A Mo4 93.80(9) 1_545 1_546 ?
O1 Ba1A Mo4 72.74(6) 1_545 2_545 ?
O1 Ba1A O1 94.77(16) 2_546 1_545 ?
O2 Ba1A Mo2 164.16(10) 2_556 3_656 ?
O2 Ba1A Mo2 164.16(10) . 4_556 ?
O2 Ba1A Mo2 33.14(4) 2_556 4_556 ?
O2 Ba1A Mo2 33.14(4) . 3_656 ?
O2 Ba1A Mo4 107.73(4) 2_556 2_545 ?
O2 Ba1A Mo4 107.73(4) . 1_546 ?
O2 Ba1A Mo4 78.90(4) 2_556 1_546 ?
O2 Ba1A Mo4 78.90(4) . 2_545 ?
O2 Ba1A O1 61.83(6) . 1_545 ?
O2 Ba1A O1 61.83(6) 2_556 2_546 ?
O2 Ba1A O1 156.58(19) 2_556 1_545 ?
O2 Ba1A O1 156.58(19) . 2_546 ?
O2 Ba1A O2 141.6(2) 2_556 . ?
O2 Ba1A O5 103.47(7) 2_556 4_556 ?
O2 Ba1A O5 103.47(7) . 3_656 ?
O2 Ba1A O5 101.41(7) . 4_556 ?
O2 Ba1A O5 101.41(7) 2_556 3_656 ?
O2 Ba1A O6 82.75(8) . 4_566 ?
O2 Ba1A O6 84.19(9) . 3_666 ?
O2 Ba1A O6 84.19(9) 2_556 4_566 ?
O2 Ba1A O6 82.75(8) 2_556 3_666 ?
O5 Ba1A Mo2 92.16(8) 4_556 3_656 ?
O5 Ba1A Mo2 73.38(6) 4_556 4_556 ?
O5 Ba1A Mo2 73.38(6) 3_656 3_656 ?
O5 Ba1A Mo2 92.16(8) 3_656 4_556 ?
O5 Ba1A Mo4 33.50(3) 4_556 2_545 ?
O5 Ba1A Mo4 127.66(16) 4_556 1_546 ?
O5 Ba1A Mo4 33.50(3) 3_656 1_546 ?
O5 Ba1A Mo4 127.66(16) 3_656 2_545 ?
O5 Ba1A O1 63.93(10) 3_656 1_545 ?
O5 Ba1A O1 63.43(10) 4_556 1_545 ?
O5 Ba1A O1 63.93(10) 4_556 2_546 ?
O5 Ba1A O1 63.43(10) 3_656 2_546 ?
O5 Ba1A O5 98.19(17) 4_556 3_656 ?
O6 Ba1A Mo2 106.01(4) 3_666 4_556 ?
O6 Ba1A Mo2 81.68(3) 3_666 3_656 ?
O6 Ba1A Mo2 106.01(4) 4_566 3_656 ?
O6 Ba1A Mo2 81.68(3) 4_566 4_556 ?
O6 Ba1A Mo4 162.43(11) 3_666 2_545 ?
O6 Ba1A Mo4 33.31(4) 3_666 1_546 ?
O6 Ba1A Mo4 33.31(4) 4_566 2_545 ?
O6 Ba1A Mo4 162.43(11) 4_566 1_546 ?
O6 Ba1A O1 103.67(7) 3_666 2_546 ?
O6 Ba1A O1 103.39(7) 3_666 1_545 ?
O6 Ba1A O1 103.39(7) 4_566 2_546 ?
O6 Ba1A O1 103.67(7) 4_566 1_545 ?
O6 Ba1A O5 61.12(5) 4_566 4_556 ?
O6 Ba1A O5 159.30(19) 4_566 3_656 ?
O6 Ba1A O5 159.30(19) 3_666 4_556 ?
O6 Ba1A O5 61.12(5) 3_666 3_656 ?
O6 Ba1A O6 139.6(2) 3_666 4_566 ?
Mo2 Ba1B Mo2 167.3(2) 4_556 3_656 ?
Mo2 Ba1B Mo4 90.90(3) 3_656 1_546 ?
Mo2 Ba1B Mo4 87.95(2) 3_656 2_545 ?
Mo2 Ba1B Mo4 87.95(2) 4_556 1_546 ?
Mo2 Ba1B Mo4 90.90(3) 4_556 2_545 ?
Mo4 Ba1B Mo4 169.6(2) 2_545 1_546 ?
O1 Ba1B Mo2 33.81(3) 1_545 3_656 ?
O1 Ba1B Mo2 33.81(3) 2_546 4_556 ?
O1 Ba1B Mo2 134.0(2) 2_546 3_656 ?
O1 Ba1B Mo2 134.0(2) 1_545 4_556 ?
O1 Ba1B Mo4 98.06(11) 2_546 2_545 ?
O1 Ba1B Mo4 98.06(11) 1_545 1_546 ?
O1 Ba1B Mo4 75.38(7) 2_546 1_546 ?
O1 Ba1B Mo4 75.38(7) 1_545 2_545 ?
O1 Ba1B O1 103.9(3) 2_546 1_545 ?
O1 Ba1B O2 63.13(5) 1_545 . ?
O1 Ba1B O2 63.13(5) 2_546 2_556 ?
O1 Ba1B O2 167.0(3) 2_546 . ?
O1 Ba1B O2 167.0(3) 1_545 2_556 ?
O1 Ba1B O6 105.45(6) 1_545 3_666 ?
O1 Ba1B O6 105.45(6) 2_546 4_566 ?
O1 Ba1B O6 105.74(6) 1_545 4_566 ?
O1 Ba1B O6 105.74(6) 2_546 3_666 ?
O2 Ba1B Mo2 34.26(4) 2_556 4_556 ?
O2 Ba1B Mo2 34.26(4) . 3_656 ?
O2 Ba1B Mo2 157.0(2) 2_556 3_656 ?
O2 Ba1B Mo2 157.0(2) . 4_556 ?
O2 Ba1B Mo4 106.23(7) 2_556 2_545 ?
O2 Ba1B Mo4 78.33(4) . 2_545 ?
O2 Ba1B Mo4 106.23(7) . 1_546 ?
O2 Ba1B Mo4 78.33(4) 2_556 1_546 ?
O2 Ba1B O2 129.8(3) 2_556 . ?
O2 Ba1B O6 80.01(13) . 3_666 ?
O2 Ba1B O6 80.01(13) 2_556 4_566 ?
O2 Ba1B O6 78.67(12) . 4_566 ?
O2 Ba1B O6 78.67(12) 2_556 3_666 ?
O5 Ba1B Mo2 96.30(11) 4_556 3_656 ?
O5 Ba1B Mo2 96.30(11) 3_656 4_556 ?
O5 Ba1B Mo2 76.10(7) 3_656 3_656 ?
O5 Ba1B Mo2 76.10(7) 4_556 4_556 ?
O5 Ba1B Mo4 33.51(4) 3_656 1_546 ?
O5 Ba1B Mo4 136.6(2) 4_556 1_546 ?
O5 Ba1B Mo4 33.51(4) 4_556 2_545 ?
O5 Ba1B Mo4 136.6(2) 3_656 2_545 ?
O5 Ba1B O1 68.42(14) 4_556 1_545 ?
O5 Ba1B O1 68.97(14) 4_556 2_546 ?
O5 Ba1B O1 68.97(14) 3_656 1_545 ?
O5 Ba1B O1 68.42(14) 3_656 2_546 ?
O5 Ba1B O2 105.54(6) 4_556 2_556 ?
O5 Ba1B O2 103.42(6) 4_556 . ?
O5 Ba1B O2 103.42(6) 3_656 2_556 ?
O5 Ba1B O2 105.54(6) 3_656 . ?
O5 Ba1B O5 107.7(3) 4_556 3_656 ?
O5 Ba1B O6 169.7(3) 3_656 4_566 ?
O5 Ba1B O6 62.01(5) 3_656 3_666 ?
O5 Ba1B O6 62.01(5) 4_556 4_566 ?
O5 Ba1B O6 169.7(3) 4_556 3_666 ?
O6 Ba1B Mo2 104.62(6) 4_566 3_656 ?
O6 Ba1B Mo2 81.04(4) 3_666 3_656 ?
O6 Ba1B Mo2 81.04(4) 4_566 4_556 ?
O6 Ba1B Mo2 104.62(6) 3_666 4_556 ?
O6 Ba1B Mo4 155.0(2) 4_566 1_546 ?
O6 Ba1B Mo4 34.21(4) 4_566 2_545 ?
O6 Ba1B Mo4 155.0(2) 3_666 2_545 ?
O6 Ba1B Mo4 34.21(4) 3_666 1_546 ?
O6 Ba1B O6 128.3(3) 3_666 4_566 ?
Mo1 Ba2A Mo1 160.41(14) 3_666 4_566 ?
Mo1 Ba2A Mo3 86.94(2) 4_566 1_556 ?
Mo1 Ba2A Mo3 86.94(2) 3_666 2 ?
Mo1 Ba2A Mo3 89.27(3) 3_666 1_556 ?
Mo1 Ba2A Mo3 89.27(3) 4_566 2 ?
Mo3 Ba2A Mo3 157.61(14) 1_556 2 ?
O1 Ba2A Mo1 128.16(14) 2_556 3_666 ?
O1 Ba2A Mo1 32.62(3) 2_556 4_566 ?
O1 Ba2A Mo1 32.62(3) . 3_666 ?
O1 Ba2A Mo1 128.16(14) . 4_566 ?
O1 Ba2A Mo3 90.72(7) . 1_556 ?
O1 Ba2A Mo3 74.42(6) . 2 ?
O1 Ba2A Mo3 90.72(7) 2_556 2 ?
O1 Ba2A Mo3 74.42(6) 2_556 1_556 ?
O1 Ba2A O1 97.49(15) 2_556 . ?
O1 Ba2A O5 63.88(9) . 3_666 ?
O1 Ba2A O5 63.38(9) . 4_566 ?
O1 Ba2A O5 63.88(9) 2_556 4_566 ?
O1 Ba2A O5 63.38(9) 2_556 3_666 ?
O2 Ba2A Mo1 165.21(12) . 4_566 ?
O2 Ba2A Mo1 31.93(4) . 3_666 ?
O2 Ba2A Mo1 165.21(12) 2_556 3_666 ?
O2 Ba2A Mo1 31.93(4) 2_556 4_566 ?
O2 Ba2A Mo3 82.90(4) 2_556 1_556 ?
O2 Ba2A Mo3 82.89(4) . 2 ?
O2 Ba2A Mo3 104.98(4) 2_556 2 ?
O2 Ba2A Mo3 104.98(4) . 1_556 ?
O2 Ba2A O1 61.58(5) . . ?
O2 Ba2A O1 159.05(17) 2_556 . ?
O2 Ba2A O1 159.05(17) . 2_556 ?
O2 Ba2A O1 61.58(5) 2_556 2_556 ?
O2 Ba2A O2 139.4(2) 2_556 . ?
O2 Ba2A O5 102.53(6) . 4_566 ?
O2 Ba2A O5 104.53(6) 2_556 4_566 ?
O2 Ba2A O5 102.53(6) 2_556 3_666 ?
O2 Ba2A O5 104.53(6) . 3_666 ?
O2 Ba2A O6 82.97(8) . 4_566 ?
O2 Ba2A O6 84.41(8) 2_556 4_566 ?
O2 Ba2A O6 82.97(8) 2_556 3_666 ?
O2 Ba2A O6 84.41(8) . 3_666 ?
O5 Ba2A Mo1 90.24(7) 3_666 4_566 ?
O5 Ba2A Mo1 90.24(7) 4_566 3_666 ?
O5 Ba2A Mo1 76.51(6) 4_566 4_566 ?
O5 Ba2A Mo1 76.51(6) 3_666 3_666 ?
O5 Ba2A Mo3 125.59(13) 4_566 1_556 ?
O5 Ba2A Mo3 125.59(13) 3_666 2 ?
O5 Ba2A Mo3 32.49(3) 3_666 1_556 ?
O5 Ba2A Mo3 32.49(3) 4_566 2 ?
O5 Ba2A O5 95.31(14) 3_666 4_566 ?
O6 Ba2A Mo1 83.79(3) 4_566 4_566 ?
O6 Ba2A Mo1 83.79(3) 3_666 3_666 ?
O6 Ba2A Mo1 102.46(3) 3_666 4_566 ?
O6 Ba2A Mo1 102.46(3) 4_566 3_666 ?
O6 Ba2A Mo3 166.99(9) 4_566 1_556 ?
O6 Ba2A Mo3 166.99(9) 3_666 2 ?
O6 Ba2A Mo3 31.63(4) 4_566 2 ?
O6 Ba2A Mo3 31.63(4) 3_666 1_556 ?
O6 Ba2A O1 101.91(6) 4_566 2_556 ?
O6 Ba2A O1 101.91(6) 3_666 . ?
O6 Ba2A O1 102.19(6) 3_666 2_556 ?
O6 Ba2A O1 102.19(6) 4_566 . ?
O6 Ba2A O5 156.10(16) 3_666 4_566 ?
O6 Ba2A O5 60.80(5) 3_666 3_666 ?
O6 Ba2A O5 60.80(5) 4_566 4_566 ?
O6 Ba2A O5 156.10(16) 4_566 3_666 ?
O6 Ba2A O6 143.10(19) 4_566 3_666 ?
Mo1 Ba2B Mo1 169.4(3) 3_666 4_566 ?
Mo1 Ba2B Mo3 90.57(3) 3_666 1_556 ?
Mo1 Ba2B Mo3 88.19(3) 4_566 1_556 ?
Mo1 Ba2B Mo3 88.19(3) 3_666 2 ?
Mo1 Ba2B Mo3 90.57(3) 4_566 2 ?
Mo3 Ba2B Mo3 166.5(3) 1_556 2 ?
O1 Ba2B Mo1 32.52(4) 2_556 4_566 ?
O1 Ba2B Mo1 137.2(3) . 4_566 ?
O1 Ba2B Mo1 32.52(4) . 3_666 ?
O1 Ba2B Mo1 137.2(3) 2_556 3_666 ?
O1 Ba2B Mo3 94.71(14) . 1_556 ?
O1 Ba2B Mo3 77.17(10) . 2 ?
O1 Ba2B Mo3 77.17(10) 2_556 1_556 ?
O1 Ba2B Mo3 94.71(14) 2_556 2 ?
O1 Ba2B O1 106.9(4) 2_556 . ?
O1 Ba2B O2 62.59(5) 2_556 2_556 ?
O1 Ba2B O2 169.4(4) 2_556 . ?
O1 Ba2B O2 169.4(4) . 2_556 ?
O1 Ba2B O2 62.59(5) . . ?
O1 Ba2B O5 68.84(19) 2_556 4_566 ?
O1 Ba2B O5 68.84(19) . 3_666 ?
O1 Ba2B O5 68.29(19) . 4_566 ?
O1 Ba2B O5 68.29(19) 2_556 3_666 ?
O1 Ba2B O6 104.27(7) 2_556 3_666 ?
O1 Ba2B O6 103.97(7) . 3_666 ?
O1 Ba2B O6 104.26(7) . 4_566 ?
O1 Ba2B O6 103.97(7) 2_556 4_566 ?
O2 Ba2B Mo1 156.8(3) 2_556 3_666 ?
O2 Ba2B Mo1 33.02(4) 2_556 4_566 ?
O2 Ba2B Mo1 33.02(4) . 3_666 ?
O2 Ba2B Mo1 156.8(3) . 4_566 ?
O2 Ba2B Mo3 82.31(5) . 2 ?
O2 Ba2B Mo3 103.71(7) 2_556 2 ?
O2 Ba2B Mo3 103.71(7) . 1_556 ?
O2 Ba2B Mo3 82.31(5) 2_556 1_556 ?
O2 Ba2B O2 127.9(4) 2_556 . ?
O2 Ba2B O6 80.32(16) 2_556 4_566 ?
O2 Ba2B O6 78.97(16) 2_556 3_666 ?
O2 Ba2B O6 80.32(16) . 3_666 ?
O2 Ba2B O6 78.97(16) . 4_566 ?
O5 Ba2B Mo1 94.10(14) 3_666 4_566 ?
O5 Ba2B Mo1 79.35(10) 3_666 3_666 ?
O5 Ba2B Mo1 94.10(14) 4_566 3_666 ?
O5 Ba2B Mo1 79.35(10) 4_566 4_566 ?
O5 Ba2B Mo3 32.55(3) 4_566 2 ?
O5 Ba2B Mo3 134.3(3) 3_666 2 ?
O5 Ba2B Mo3 134.3(3) 4_566 1_556 ?
O5 Ba2B Mo3 32.55(3) 3_666 1_556 ?
O5 Ba2B O2 104.59(7) 4_566 . ?
O5 Ba2B O2 104.59(7) 3_666 2_556 ?
O5 Ba2B O2 106.66(7) 3_666 . ?
O5 Ba2B O2 106.66(7) 4_566 2_556 ?
O5 Ba2B O5 104.3(3) 3_666 4_566 ?
O5 Ba2B O6 62.03(5) 4_566 4_566 ?
O5 Ba2B O6 166.3(4) 3_666 4_566 ?
O5 Ba2B O6 62.03(5) 3_666 3_666 ?
O5 Ba2B O6 166.3(4) 4_566 3_666 ?
O6 Ba2B Mo1 101.26(7) 3_666 4_566 ?
O6 Ba2B Mo1 83.13(5) 4_566 4_566 ?
O6 Ba2B Mo1 101.26(7) 4_566 3_666 ?
O6 Ba2B Mo1 83.13(5) 3_666 3_666 ?
O6 Ba2B Mo3 32.79(5) 4_566 2 ?
O6 Ba2B Mo3 32.79(5) 3_666 1_556 ?
O6 Ba2B Mo3 159.5(3) 3_666 2 ?
O6 Ba2B Mo3 159.5(3) 4_566 1_556 ?
O6 Ba2B O6 131.6(4) 4_566 3_666 ?
Mo1 Mo1 Ba2A 84.93(4) 3_666 3_666 ?
Mo1 Mo1 Ba2B 82.46(9) 3_666 3_666 ?
Mo1 Mo1 Mo2 59.717(9) 3_666 3_666 ?
Mo1 Mo1 Mo2 125.251(11) 3_666 1_565 ?
Mo1 Mo1 Mo2 62.549(8) 3_666 . ?
Mo2 Mo1 Ba2A 79.54(7) 1_565 3_666 ?
Mo2 Mo1 Ba2A 76.39(3) 3_666 3_666 ?
Mo2 Mo1 Ba2A 98.93(7) . 3_666 ?
Mo2 Mo1 Ba2B 84.04(16) 1_565 3_666 ?
Mo2 Mo1 Ba2B 94.44(16) . 3_666 ?
Mo2 Mo1 Ba2B 78.44(8) 3_666 3_666 ?
Mo2 Mo1 Mo2 171.556(10) . 1_565 ?
Mo2 Mo1 Mo2 65.631(7) 3_666 1_565 ?
Mo2 Mo1 Mo2 122.265(8) . 3_666 ?
O1 Mo1 Ba2A 49.97(8) 3_666 3_666 ?
O1 Mo1 Ba2A 122.17(5) . 3_666 ?
O1 Mo1 Ba2B 122.40(5) . 3_666 ?
O1 Mo1 Ba2B 45.61(16) 3_666 3_666 ?
O1 Mo1 Mo1 51.76(5) . 3_666 ?
O1 Mo1 Mo1 51.95(5) 3_666 3_666 ?
O1 Mo1 Mo2 90.82(5) 3_666 3_666 ?
O1 Mo1 Mo2 51.81(5) 3_666 . ?
O1 Mo1 Mo2 128.69(5) 3_666 1_565 ?
O1 Mo1 Mo2 50.48(5) . 3_666 ?
O1 Mo1 Mo2 92.74(5) . . ?
O1 Mo1 Mo2 95.08(4) . 1_565 ?
O1 Mo1 O1 103.71(6) 3_666 . ?
O1 Mo1 O2 88.67(6) 3_666 3_666 ?
O1 Mo1 O2 98.66(6) . 3_666 ?
O1 Mo1 O3 172.59(7) . . ?
O1 Mo1 O3 82.10(7) 3_666 . ?
O1 Mo1 O8 89.13(7) . 2 ?
O1 Mo1 O8 165.86(7) 3_666 2 ?
O2 Mo1 Ba2A 43.61(8) 3_666 3_666 ?
O2 Mo1 Ba2B 47.87(16) 3_666 3_666 ?
O2 Mo1 Mo1 95.93(5) 3_666 3_666 ?
O2 Mo1 Mo2 49.30(5) 3_666 3_666 ?
O2 Mo1 Mo2 140.47(4) 3_666 . ?
O2 Mo1 Mo2 40.98(4) 3_666 1_565 ?
O2 Mo1 O3 85.94(7) 3_666 . ?
O2 Mo1 O8 83.51(6) 3_666 2 ?
O3 Mo1 Ba2A 65.08(5) . 3_666 ?
O3 Mo1 Ba2B 64.96(5) . 3_666 ?
O3 Mo1 Mo1 133.85(5) . 3_666 ?
O3 Mo1 Mo2 84.56(5) . 1_565 ?
O3 Mo1 Mo2 134.95(5) . 3_666 ?
O3 Mo1 Mo2 87.27(5) . . ?
O3 Mo1 O8 85.61(7) . 2 ?
O7 Mo1 Ba2A 139.17(7) . 3_666 ?
O7 Mo1 Ba2B 135.43(14) . 3_666 ?
O7 Mo1 Mo1 94.98(5) . 3_666 ?
O7 Mo1 Mo2 137.57(5) . 3_666 ?
O7 Mo1 Mo2 129.55(5) . 1_565 ?
O7 Mo1 Mo2 47.67(4) . . ?
O7 Mo1 O1 87.12(7) . . ?
O7 Mo1 O1 99.08(7) . 3_666 ?
O7 Mo1 O2 169.02(7) . 3_666 ?
O7 Mo1 O3 87.42(7) . . ?
O7 Mo1 O8 87.27(7) . 2 ?
O8 Mo1 Ba2A 117.96(8) 2 3_666 ?
O8 Mo1 Ba2B 122.10(16) 2 3_666 ?
O8 Mo1 Mo1 140.51(5) 2 3_666 ?
O8 Mo1 Mo2 42.52(4) 2 1_565 ?
O8 Mo1 Mo2 92.95(5) 2 3_666 ?
O8 Mo1 Mo2 134.66(4) 2 . ?
Ba1B Mo2 Na1B 0.0(2) 3_656 3_656 ?
Mo1 Mo2 Ba1B 84.14(12) 1_545 3_656 ?
Mo1 Mo2 Ba1B 81.18(6) 3_666 3_656 ?
Mo1 Mo2 Ba1B 96.90(12) . 3_656 ?
Mo1 Mo2 Na1B 84.14(12) 1_545 3_656 ?
Mo1 Mo2 Na1B 96.90(12) . 3_656 ?
Mo1 Mo2 Na1B 81.18(6) 3_666 3_656 ?
Mo1 Mo2 Mo1 57.734(8) . 3_666 ?
Mo1 Mo2 Mo1 114.370(7) 3_666 1_545 ?
Mo1 Mo2 Mo1 171.556(10) . 1_545 ?
Mo1 Mo2 Mo2 49.478(6) 1_545 3_656 ?
Mo1 Mo2 Mo2 64.892(8) 3_666 3_656 ?
Mo1 Mo2 Mo2 122.534(10) . 3_656 ?
Mo2 Mo2 Ba1B 76.73(7) 3_656 3_656 ?
Mo2 Mo2 Na1B 76.73(7) 3_656 3_656 ?
O1 Mo2 Ba1B 47.90(12) 3_666 3_656 ?
O1 Mo2 Na1B 47.90(12) 3_666 3_656 ?
O1 Mo2 Mo1 127.89(4) 3_666 1_545 ?
O1 Mo2 Mo1 49.52(5) 3_666 3_666 ?
O1 Mo2 Mo1 50.63(4) 3_666 . ?
O1 Mo2 Mo2 93.94(5) 3_666 3_656 ?
O1 Mo2 O2 87.99(6) 3_666 3_656 ?
O1 Mo2 O8 169.48(6) 3_666 2_545 ?
O2 Mo2 Ba1B 109.33(5) . 3_656 ?
O2 Mo2 Ba1B 48.03(12) 3_656 3_656 ?
O2 Mo2 Na1B 48.03(12) 3_656 3_656 ?
O2 Mo2 Na1B 109.33(5) . 3_656 ?
O2 Mo2 Mo1 39.91(4) 3_656 1_545 ?
O2 Mo2 Mo1 77.08(4) . 1_545 ?
O2 Mo2 Mo1 94.71(4) . . ?
O2 Mo2 Mo1 49.83(5) . 3_666 ?
O2 Mo2 Mo1 89.04(5) 3_656 3_666 ?
O2 Mo2 Mo1 137.29(5) 3_656 . ?
O2 Mo2 Mo2 40.49(4) . 3_656 ?
O2 Mo2 Mo2 39.06(5) 3_656 3_656 ?
O2 Mo2 O1 98.25(7) . 3_666 ?
O2 Mo2 O2 79.55(7) . 3_656 ?
O2 Mo2 O8 81.31(7) . 2_545 ?
O2 Mo2 O8 81.58(6) 3_656 2_545 ?
O4 Mo2 Ba1B 66.07(5) . 3_656 ?
O4 Mo2 Na1B 66.07(5) . 3_656 ?
O4 Mo2 Mo1 101.45(5) . . ?
O4 Mo2 Mo1 86.65(5) . 1_545 ?
O4 Mo2 Mo1 139.30(5) . 3_666 ?
O4 Mo2 Mo2 125.07(5) . 3_656 ?
O4 Mo2 O1 89.86(7) . 3_666 ?
O4 Mo2 O2 163.57(6) . . ?
O4 Mo2 O2 86.52(7) . 3_656 ?
O4 Mo2 O8 88.11(7) . 2_545 ?
O7 Mo2 Ba1B 142.18(12) . 3_656 ?
O7 Mo2 Na1B 142.18(12) . 3_656 ?
O7 Mo2 Mo1 93.57(5) . 3_666 ?
O7 Mo2 Mo1 51.03(5) . . ?
O7 Mo2 Mo1 130.77(5) . 1_545 ?
O7 Mo2 Mo2 134.52(5) . 3_656 ?
O7 Mo2 O1 101.23(7) . 3_666 ?
O7 Mo2 O2 169.77(6) . 3_656 ?
O7 Mo2 O2 94.60(7) . . ?
O7 Mo2 O4 97.82(7) . . ?
O7 Mo2 O8 89.28(7) . 2_545 ?
O8 Mo2 Ba1B 122.23(13) 2_545 3_656 ?
O8 Mo2 Na1B 122.23(13) 2_545 3_656 ?
O8 Mo2 Mo1 41.68(4) 2_545 1_545 ?
O8 Mo2 Mo1 131.14(5) 2_545 3_666 ?
O8 Mo2 Mo1 139.87(4) 2_545 . ?
O8 Mo2 Mo2 78.85(5) 2_545 3_656 ?
Mo3 Mo3 Ba2A 82.35(3) 3_665 1_554 ?
Mo3 Mo3 Ba2B 80.21(8) 3_665 1_554 ?
Mo3 Mo3 Mo4 120.322(10) 3_665 1_545 ?
Mo3 Mo3 Mo4 56.243(8) 3_665 3_665 ?
Mo3 Mo3 Mo4 68.151(9) 3_665 . ?
Mo4 Mo3 Ba2A 78.18(7) 1_545 1_554 ?
Mo4 Mo3 Ba2A 100.33(7) . 1_554 ?
Mo4 Mo3 Ba2A 73.80(3) 3_665 1_554 ?
Mo4 Mo3 Ba2B 82.61(16) 1_545 1_554 ?
Mo4 Mo3 Ba2B 75.92(8) 3_665 1_554 ?
Mo4 Mo3 Ba2B 95.90(16) . 1_554 ?
Mo4 Mo3 Mo4 64.198(7) 3_665 1_545 ?
Mo4 Mo3 Mo4 124.394(7) . 3_665 ?
Mo4 Mo3 Mo4 170.752(10) . 1_545 ?
O3 Mo3 Ba2A 142.47(8) . 1_554 ?
O3 Mo3 Ba2B 138.72(15) . 1_554 ?
O3 Mo3 Mo3 99.00(5) . 3_665 ?
O3 Mo3 Mo4 48.14(5) . . ?
O3 Mo3 Mo4 129.17(5) . 1_545 ?
O3 Mo3 Mo4 137.46(5) . 3_665 ?
O3 Mo3 O4 89.32(7) . . ?
O3 Mo3 O5 90.74(7) . . ?
O3 Mo3 O5 100.39(7) . 3_665 ?
O3 Mo3 O6 169.38(7) . 3_665 ?
O3 Mo3 O7 89.71(7) . 2 ?
O4 Mo3 Ba2A 115.55(8) . 1_554 ?
O4 Mo3 Ba2B 119.74(16) . 1_554 ?
O4 Mo3 Mo3 136.43(5) . 3_665 ?
O4 Mo3 Mo4 40.12(5) . 1_545 ?
O4 Mo3 Mo4 89.35(5) . 3_665 ?
O4 Mo3 Mo4 137.03(5) . . ?
O5 Mo3 Ba2A 117.40(5) . 1_554 ?
O5 Mo3 Ba2A 51.37(8) 3_665 1_554 ?
O5 Mo3 Ba2B 47.07(16) 3_665 1_554 ?
O5 Mo3 Ba2B 118.11(5) . 1_554 ?
O5 Mo3 Mo3 51.85(5) . 3_665 ?
O5 Mo3 Mo3 51.79(5) 3_665 3_665 ?
O5 Mo3 Mo4 98.70(5) . . ?
O5 Mo3 Mo4 89.86(5) 3_665 3_665 ?
O5 Mo3 Mo4 90.00(5) . 1_545 ?
O5 Mo3 Mo4 46.78(5) . 3_665 ?
O5 Mo3 Mo4 128.60(5) 3_665 1_545 ?
O5 Mo3 Mo4 52.33(5) 3_665 . ?
O5 Mo3 O4 166.38(7) 3_665 . ?
O5 Mo3 O4 85.61(7) . . ?
O5 Mo3 O5 103.64(6) . 3_665 ?
O5 Mo3 O6 91.06(6) . 3_665 ?
O5 Mo3 O6 89.35(7) 3_665 3_665 ?
O6 Mo3 Ba2A 43.63(8) 3_665 1_554 ?
O6 Mo3 Ba2B 47.81(16) 3_665 1_554 ?
O6 Mo3 Mo3 90.33(4) 3_665 3_665 ?
O6 Mo3 Mo4 141.66(5) 3_665 . ?
O6 Mo3 Mo4 40.37(5) 3_665 1_545 ?
O6 Mo3 Mo4 45.78(5) 3_665 3_665 ?
O6 Mo3 O4 80.38(6) 3_665 . ?
O7 Mo3 Ba2A 66.09(5) 2 1_554 ?
O7 Mo3 Ba2B 66.01(5) 2 1_554 ?
O7 Mo3 Mo3 136.22(5) 2 3_665 ?
O7 Mo3 Mo4 132.58(5) 2 3_665 ?
O7 Mo3 Mo4 83.28(5) 2 1_545 ?
O7 Mo3 Mo4 87.78(5) 2 . ?
O7 Mo3 O4 86.07(7) 2 . ?
O7 Mo3 O5 84.46(7) 2 3_665 ?
O7 Mo3 O5 171.66(7) 2 . ?
O7 Mo3 O6 87.02(7) 2 3_665 ?
Ba1B Mo4 Na1B 0.0(2) 1_564 1_564 ?
Mo3 Mo4 Ba1A 81.35(4) 3_665 1_564 ?
Mo3 Mo4 Ba1A 100.27(8) . 1_564 ?
Mo3 Mo4 Ba1A 80.63(8) 1_565 1_564 ?
Mo3 Mo4 Ba1B 78.93(6) 3_665 1_564 ?
Mo3 Mo4 Ba1B 95.71(12) . 1_564 ?
Mo3 Mo4 Ba1B 85.20(12) 1_565 1_564 ?
Mo3 Mo4 Na1B 85.20(12) 1_565 1_564 ?
Mo3 Mo4 Na1B 95.71(12) . 1_564 ?
Mo3 Mo4 Na1B 78.93(6) 3_665 1_564 ?
Mo3 Mo4 Mo3 55.606(8) . 3_665 ?
Mo3 Mo4 Mo3 115.801(7) 3_665 1_565 ?
Mo3 Mo4 Mo3 170.751(10) . 1_565 ?
O3 Mo4 Ba1A 146.74(9) . 1_564 ?
O3 Mo4 Ba1B 142.42(13) . 1_564 ?
O3 Mo4 Na1B 142.42(13) . 1_564 ?
O3 Mo4 Mo3 130.98(5) . 1_565 ?
O3 Mo4 Mo3 50.50(5) . . ?
O3 Mo4 Mo3 90.78(5) . 3_665 ?
O3 Mo4 O4 90.57(7) . 1_565 ?
O3 Mo4 O5 101.73(7) . 3_665 ?
O3 Mo4 O6 167.00(7) . 3_675 ?
O3 Mo4 O6 92.40(7) . . ?
O4 Mo4 Ba1A 118.91(9) 1_565 1_564 ?
O4 Mo4 Ba1B 123.41(13) 1_565 1_564 ?
O4 Mo4 Na1B 123.41(13) 1_565 1_564 ?
O4 Mo4 Mo3 40.66(5) 1_565 1_565 ?
O4 Mo4 Mo3 130.94(5) 1_565 3_665 ?
O4 Mo4 Mo3 140.55(5) 1_565 . ?
O4 Mo4 O5 167.03(6) 1_565 3_665 ?
O4 Mo4 O6 80.05(6) 1_565 3_675 ?
O5 Mo4 Ba1A 50.71(9) 3_665 1_564 ?
O5 Mo4 Ba1B 46.41(12) 3_665 1_564 ?
O5 Mo4 Na1B 46.41(12) 3_665 1_564 ?
O5 Mo4 Mo3 126.63(5) 3_665 1_565 ?
O5 Mo4 Mo3 45.89(5) 3_665 3_665 ?
O5 Mo4 Mo3 51.30(5) 3_665 . ?
O5 Mo4 O6 87.15(7) 3_665 3_675 ?
O6 Mo4 Ba1A 45.82(9) 3_675 1_564 ?
O6 Mo4 Ba1A 104.55(5) . 1_564 ?
O6 Mo4 Ba1B 49.97(12) 3_675 1_564 ?
O6 Mo4 Ba1B 105.14(5) . 1_564 ?
O6 Mo4 Na1B 105.14(5) . 1_564 ?
O6 Mo4 Na1B 49.97(12) 3_675 1_564 ?
O6 Mo4 Mo3 39.49(5) 3_675 1_565 ?
O6 Mo4 Mo3 136.88(4) 3_675 . ?
O6 Mo4 Mo3 46.19(5) . 3_665 ?
O6 Mo4 Mo3 88.66(4) 3_675 3_665 ?
O6 Mo4 Mo3 90.11(4) . . ?
O6 Mo4 Mo3 80.78(4) . 1_565 ?
O6 Mo4 O4 84.76(7) . 1_565 ?
O6 Mo4 O5 90.59(7) . 3_665 ?
O6 Mo4 O6 77.89(7) . 3_675 ?
O8 Mo4 Ba1A 66.66(5) . 1_564 ?
O8 Mo4 Ba1B 66.97(5) . 1_564 ?
O8 Mo4 Na1B 66.97(5) . 1_564 ?
O8 Mo4 Mo3 137.02(5) . 3_665 ?
O8 Mo4 Mo3 101.41(5) . . ?
O8 Mo4 Mo3 87.43(5) . 1_565 ?
O8 Mo4 O3 100.40(7) . . ?
O8 Mo4 O4 90.65(7) . 1_565 ?
O8 Mo4 O5 91.12(7) . 3_665 ?
O8 Mo4 O6 166.46(7) . . ?
O8 Mo4 O6 88.78(7) . 3_675 ?
Na1A O1 Ba1A 0.0 1_565 1_565 ?
Na1B O1 Ba1B 0.0 1_565 1_565 ?
Mo1 O1 Ba1A 161.98(8) 3_666 1_565 ?
Mo1 O1 Ba1A 118.39(8) . 1_565 ?
Mo1 O1 Na1A 118.39(8) . 1_565 ?
Mo1 O1 Na1A 161.98(8) 3_666 1_565 ?
Mo1 O1 Ba1B 120.79(10) . 1_565 ?
Mo1 O1 Ba1B 161.83(9) 3_666 1_565 ?
Mo1 O1 Na1B 161.83(9) 3_666 1_565 ?
Mo1 O1 Na1B 120.79(10) . 1_565 ?
Mo1 O1 Ba2A 121.51(8) . . ?
Mo1 O1 Ba2A 97.40(9) 3_666 . ?
Mo1 O1 Ba2B 101.87(18) 3_666 . ?
Mo1 O1 Ba2B 123.75(11) . . ?
Mo1 O1 Mo1 76.29(6) 3_666 . ?
Mo1 O1 Mo2 80.00(6) . 3_666 ?
Mo1 O1 Mo2 77.56(6) 3_666 3_666 ?
Mo2 O1 Ba1A 94.10(9) 3_666 1_565 ?
Mo2 O1 Na1A 94.10(9) 3_666 1_565 ?
Mo2 O1 Ba1B 98.29(13) 3_666 1_565 ?
Mo2 O1 Na1B 98.29(13) 3_666 1_565 ?
Mo2 O1 Ba2A 156.52(8) 3_666 . ?
Mo2 O1 Ba2B 155.77(9) 3_666 . ?
Mo1 O2 Ba1A 140.37(12) 3_666 . ?
Mo1 O2 Ba1B 145.24(14) 3_666 . ?
Mo1 O2 Ba2A 104.46(11) 3_666 . ?
Mo1 O2 Ba2B 99.10(19) 3_666 . ?
Mo1 O2 Mo2 99.11(7) 3_666 3_656 ?
Mo2 O2 Ba1A 125.81(8) . . ?
Mo2 O2 Ba1A 103.02(12) 3_656 . ?
Mo2 O2 Ba1B 125.35(8) . . ?
Mo2 O2 Ba1B 97.72(15) 3_656 . ?
Mo2 O2 Ba2A 137.08(10) 3_656 . ?
Mo2 O2 Ba2A 118.22(8) . . ?
Mo2 O2 Ba2B 115.85(11) . . ?
Mo2 O2 Ba2B 141.42(16) 3_656 . ?
Mo2 O2 Mo1 80.87(6) . 3_666 ?
Mo2 O2 Mo2 100.45(7) . 3_656 ?
Mo3 O3 Mo1 137.64(9) . . ?
Mo4 O3 Mo1 140.94(9) . . ?
Mo4 O3 Mo3 81.36(6) . . ?
Mo2 O4 Mo3 124.19(8) . . ?
Mo2 O4 Mo4 136.36(8) . 1_545 ?
Mo4 O4 Mo3 99.23(7) 1_545 . ?
Na1A O5 Ba1A 0.0 3_656 3_656 ?
Na1B O5 Ba1B 0.0 3_656 3_656 ?
Na2A O5 Ba2A 0.0 3_666 3_666 ?
Na2B O5 Ba2B 0.0 3_666 3_666 ?
Mo3 O5 Ba1A 160.52(8) 3_665 3_656 ?
Mo3 O5 Ba1A 121.59(8) . 3_656 ?
Mo3 O5 Na1A 121.59(8) . 3_656 ?
Mo3 O5 Na1A 160.52(8) 3_665 3_656 ?
Mo3 O5 Ba1B 159.91(9) 3_665 3_656 ?
Mo3 O5 Ba1B 123.53(9) . 3_656 ?
Mo3 O5 Na1B 159.91(9) 3_665 3_656 ?
Mo3 O5 Na1B 123.53(9) . 3_656 ?
Mo3 O5 Ba2A 115.06(7) . 3_666 ?
Mo3 O5 Ba2A 96.14(9) 3_665 3_666 ?
Mo3 O5 Na2A 115.06(7) . 3_666 ?
Mo3 O5 Na2A 96.14(9) 3_665 3_666 ?
Mo3 O5 Ba2B 100.38(17) 3_665 3_666 ?
Mo3 O5 Ba2B 117.37(11) . 3_666 ?
Mo3 O5 Na2B 100.38(17) 3_665 3_666 ?
Mo3 O5 Na2B 117.37(11) . 3_666 ?
Mo3 O5 Mo3 76.36(6) . 3_665 ?
Mo3 O5 Mo4 87.32(7) . 3_665 ?
Mo3 O5 Mo4 76.37(6) 3_665 3_665 ?
Mo4 O5 Ba1A 95.79(9) 3_665 3_656 ?
Mo4 O5 Na1A 95.79(9) 3_665 3_656 ?
Mo4 O5 Ba1B 100.08(13) 3_665 3_656 ?
Mo4 O5 Na1B 100.08(13) 3_665 3_656 ?
Mo4 O5 Ba2A 154.39(8) 3_665 3_666 ?
Mo4 O5 Na2A 154.39(8) 3_665 3_666 ?
Mo4 O5 Ba2B 153.97(8) 3_665 3_666 ?
Mo4 O5 Na2B 153.97(8) 3_665 3_666 ?
Na1A O6 Ba1A 0.0 3_666 3_666 ?
Na1B O6 Ba1B 0.0 3_666 3_666 ?
Na2A O6 Ba2A 0.0 3_666 3_666 ?
Na2B O6 Ba2B 0.0 3_666 3_666 ?
Mo3 O6 Ba1A 139.61(12) 3_665 3_666 ?
Mo3 O6 Na1A 139.61(12) 3_665 3_666 ?
Mo3 O6 Ba1B 144.26(14) 3_665 3_666 ?
Mo3 O6 Na1B 144.26(14) 3_665 3_666 ?
Mo3 O6 Ba2A 104.74(11) 3_665 3_666 ?
Mo3 O6 Na2A 104.74(11) 3_665 3_666 ?
Mo3 O6 Ba2B 99.39(19) 3_665 3_666 ?
Mo3 O6 Na2B 99.39(19) 3_665 3_666 ?
Mo3 O6 Mo4 100.14(7) 3_665 3_675 ?
Mo4 O6 Ba1A 120.31(7) . 3_666 ?
Mo4 O6 Ba1A 100.87(11) 3_675 3_666 ?
Mo4 O6 Na1A 120.31(7) . 3_666 ?
Mo4 O6 Na1A 100.87(11) 3_675 3_666 ?
Mo4 O6 Ba1B 95.82(14) 3_675 3_666 ?
Mo4 O6 Ba1B 119.56(7) . 3_666 ?
Mo4 O6 Na1B 119.56(7) . 3_666 ?
Mo4 O6 Na1B 95.82(14) 3_675 3_666 ?
Mo4 O6 Ba2A 133.92(10) 3_675 3_666 ?
Mo4 O6 Ba2A 116.75(7) . 3_666 ?
Mo4 O6 Na2A 133.92(10) 3_675 3_666 ?
Mo4 O6 Na2A 116.75(7) . 3_666 ?
Mo4 O6 Ba2B 138.30(16) 3_675 3_666 ?
Mo4 O6 Ba2B 115.05(9) . 3_666 ?
Mo4 O6 Na2B 138.30(16) 3_675 3_666 ?
Mo4 O6 Na2B 115.05(9) . 3_666 ?
Mo4 O6 Mo3 88.04(6) . 3_665 ?
Mo4 O6 Mo4 102.11(7) . 3_675 ?
Mo1 O7 Mo3 136.11(8) . 2 ?
Mo2 O7 Mo1 81.30(6) . . ?
Mo2 O7 Mo3 142.58(9) . 2 ?
Mo1 O8 Mo2 95.80(6) 2 2_565 ?
Mo4 O8 Mo1 127.11(8) . 2 ?
Mo4 O8 Mo2 137.02(9) . 2_565 ?

_olex2_submission_original_sample_id EE109
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 2.353
_oxdiff_exptl_absorpt_empirical_full_min 0.759
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.9953(7)
2 0.0047(7)

_exptl_crystal_preparation       'Magnetic properties'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ee50
_database_code_depnum_ccdc_archive 'CCDC 2371928'
loop_
_audit_author_name
_audit_author_address
'Eslam M. Elbakry'
;The University of Alabama
United States of America
;
_audit_update_record             
;
2024-07-18 deposited with the CCDC.	2024-10-16 downloaded from the CCDC.
;
_audit_creation_date             2024-05-16
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6408)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            Ba1.12Mo8O16
_chemical_name_systematic        'Barium molybdenum hollandite'
_chemical_formula_moiety         'Ba1.122 Mo8 O16'
_chemical_formula_sum            'Ba1.12 Mo8 O16'
_chemical_formula_weight         1177.34
_chemical_melting_point          ?
_chemical_oxdiff_formula         'Ba1.1 Mo8 O16'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   5.73179(12)
_cell_length_b                   7.31811(17)
_cell_length_c                   7.45804(14)
_cell_angle_alpha                89.2492(17)
_cell_angle_beta                 78.4863(17)
_cell_angle_gamma                80.4477(18)
_cell_volume                     302.224(11)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    7799
_cell_measurement_temperature    301(1)
_cell_measurement_theta_max      44.8760
_cell_measurement_theta_min      2.7630
_cell_oxdiff_angle_alpha         89.2492(17)
_cell_oxdiff_angle_beta          78.4863(17)
_cell_oxdiff_angle_gamma         80.4477(18)
_cell_oxdiff_length_a            5.73179(12)
_cell_oxdiff_length_b            7.31811(17)
_cell_oxdiff_length_c            7.45804(14)
_cell_oxdiff_measurement_reflns_used 7799
_cell_oxdiff_volume              302.223(11)
_shelx_estimated_absorpt_T_max   0.800
_shelx_estimated_absorpt_T_min   0.459
_exptl_absorpt_coefficient_mu    11.689
_exptl_absorpt_correction_T_max  0.840
_exptl_absorpt_correction_T_min  0.508
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.40.16b (Rigaku Oxford Diffraction, 2018)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'lusterous dark black'
_exptl_crystal_density_diffrn    6.469
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             527
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
0 1 0 0.0053
1 0 1 0.0404
-1 0 -1 0.0228
0 -2 1 0.0148
0 2 -1 0.0053
0 2 1 0.0095
0 -1 1 0.0174
0 1 2 0.0152
1 0 0 0.0361
0 0 -1 0.0060
0 -1 -1 0.0102

_exptl_crystal_size_max          0.079
_exptl_crystal_size_mid          0.024
_exptl_crystal_size_min          0.02
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
-0.0009 0.9998 0.0011 -0.0671 0.0036 -0.0718
1.0000 0.0012 1.0010 -0.0914 -0.0118 0.1112
-1.0000 -0.0012 -1.0010 0.0914 0.0118 -0.1112
0.0013 -2.0005 0.9979 0.0999 -0.0945 0.1685
-0.0013 2.0005 -0.9979 -0.0999 0.0945 -0.1685
-0.0024 1.9988 1.0024 -0.1685 -0.0802 -0.1186
0.0004 -1.0007 0.9990 0.0328 -0.0909 0.0967
-0.0021 0.9981 2.0014 -0.1357 -0.1712 -0.0219
1.0006 0.0020 0.0009 -0.0571 0.0755 0.0863
0.0006 0.0008 -1.0001 0.0343 0.0874 -0.0249
0.0015 -0.9990 -1.0012 0.1014 0.0838 0.0469

_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0264
_diffrn_reflns_av_unetI/netI     0.0285
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.545
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            16024
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.545
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         45.008
_diffrn_reflns_theta_min         2.788
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      301.15
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean ?
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.545
_diffrn_measurement_details      
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω      3.00  79.00   0.50   45.00    --   41.85-105.00  18.00  152
  2  ω    -78.00   1.00   0.50   45.00    --  -42.79 105.00 118.00  158
  3  ω    -31.00  -5.00   0.50   45.00    --   41.85 -19.00  90.00   52
  4  ω    -24.00  31.00   0.50   45.00    --   41.85 -19.00 -30.00  110
  5  ω     14.00  42.00   0.50   45.00    --   41.85  88.00-125.08   56
  6  ω     13.00  38.00   0.50   45.00    --   41.85  92.00 -57.57   50
  7  ω    -29.00  36.00   0.50   45.00    --   41.85 -57.00 -60.00  130
  8  ω     79.00 114.00   0.50   45.00    --   41.85-178.00 -90.00   70
  9  ω    -17.00  75.00   0.50   45.00    --   41.85 -99.00  90.00  184
 10  ω     43.00  77.00   0.50   45.00    --   41.85  77.00 -90.00   68
 11  ω     51.00  77.00   0.50   45.00    --   41.85  37.00 150.00   52
 12  ω     89.00 114.00   0.50   45.00    --   41.85  37.00 150.00   50
 13  ω     25.00  75.00   0.50   45.00    --   41.85 -99.00 -30.00  100
 14  ω     13.00  39.00   0.50   45.00    --   41.85  92.00  93.24   52
 15  ω     75.00 104.00   0.50   45.00    --   41.85 178.00 -30.00   58
 16  ω    -23.00  30.00   0.50   45.00    --   41.85 -19.00-180.00  106
 17  ω     53.00  78.00   0.50   45.00    --   41.85  37.00  60.00   50
 18  ω    -21.00  10.00   0.50   45.00    --   41.85 -57.00 -30.00   62
 19  ω     27.00  59.00   0.50   45.00    --   41.85  57.00 120.00   64
 20  ω     61.00 111.00   0.50   45.00    --   41.85  57.00 120.00  100
 21  ω     40.00  65.00   0.50   45.00    --   41.85  77.00-150.00   50
 22  ω    -32.00  31.00   0.50   45.00    --   41.85 -19.00-150.00  126
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type       
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0568617000
_diffrn_orient_matrix_UB_12      -0.0671173000
_diffrn_orient_matrix_UB_13      -0.0343997000
_diffrn_orient_matrix_UB_21      0.0755625000
_diffrn_orient_matrix_UB_22      0.0037220000
_diffrn_orient_matrix_UB_23      -0.0872987000
_diffrn_orient_matrix_UB_31      0.0863833000
_diffrn_orient_matrix_UB_32      -0.0717346000
_diffrn_orient_matrix_UB_33      0.0248995000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Rotating-anode X-ray tube'
_diffrn_source_type              'Rigaku (Mo) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                4508
_reflns_number_total             4985
_reflns_odcompleteness_completeness 98.54
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     45.18
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'CrysAlisPro 1.171.40.16b (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.40.16b (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.40.16b (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2014/7 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT  (Sheldrick, 2015)'
_refine_diff_density_max         1.422
_refine_diff_density_min         -1.889
_refine_diff_density_rms         0.332
_refine_ls_extinction_coef       0.00109(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.327
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     138
_refine_ls_number_reflns         4985
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0394
_refine_ls_R_factor_gt           0.0323
_refine_ls_restrained_S_all      1.327
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+1.4285P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0542
_refine_ls_wR_factor_ref         0.0554
_refine_special_details          'Refined as a 2-component twin.,Twin'
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.99752(16)
 0.00248(16)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1A Ba 1.0000 0.0000 0.0000 0.0130(9) Uani 0.74(2) 2 d S . . A 1
Ba1B Ba 1.071(3) 0.0187(9) 0.0139(8) 0.0065(9) Uani 0.066(10) 1 d . . . A 2
Ba2 Ba 0.5923(2) -0.02740(17) -0.01957(16) 0.0090(3) Uani 0.1240(10) 1 d . . .
A 3
Mo1 Mo 0.35067(3) 0.15006(3) 0.48775(3) 0.00395(3) Uani 1 1 d . . . . .
Mo2 Mo 0.79853(3) 0.17005(3) 0.47590(3) 0.00425(3) Uani 1 1 d . . . . .
Mo3 Mo 0.44095(3) 0.49163(3) 0.84392(3) 0.00420(3) Uani 1 1 d . . . . .
Mo4 Mo 0.89350(3) 0.48111(3) 0.81555(3) 0.00448(3) Uani 1 1 d . . . . .
O1 O 0.6461(3) 0.0304(3) 0.2992(2) 0.0064(3) Uani 1 1 d . . . . .
O2 O 0.8610(3) -0.0352(2) 0.6563(2) 0.0059(2) Uani 1 1 d . . . . .
O3 O 0.6680(3) 0.6436(3) 0.7007(2) 0.0063(2) Uani 1 1 d . . . . .
O4 O 0.8351(3) 0.3668(3) 0.2848(2) 0.0063(2) Uani 1 1 d . . . . .
O5 O 0.6745(3) 0.3045(2) 0.9576(2) 0.0060(2) Uani 1 1 d . . . . .
O6 O 0.8376(3) 0.6453(3) 1.0448(2) 0.0062(2) Uani 1 1 d . . . . .
O7 O 1.0123(3) 0.2978(3) 0.6272(2) 0.0068(3) Uani 1 1 d . . . . .
O8 O 0.5144(3) 0.3083(3) 0.6303(2) 0.0061(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1A Mo2 3.6718(2) 2_755 ?
Ba1A Mo2 3.6718(2) . ?
Ba1A Mo4 3.7624(2) 1_554 ?
Ba1A Mo4 3.7624(2) 2_756 ?
Ba1A O1 2.6830(17) . ?
Ba1A O1 2.6830(17) 2_755 ?
Ba1A O2 2.8586(18) 2_756 ?
Ba1A O2 2.8586(18) 1_554 ?
Ba1A O5 2.7171(17) 1_554 ?
Ba1A O5 2.7171(17) 2_756 ?
Ba1A O6 2.8936(18) 1_544 ?
Ba1A O6 2.8936(18) 2_766 ?
Ba1B Ba1B 0.96(4) 2_755 ?
Ba1B Mo2 3.594(4) . ?
Ba1B Mo4 3.742(5) 1_554 ?
Ba1B O1 2.887(11) . ?
Ba1B O1 2.554(6) 2_755 ?
Ba1B O2 3.192(15) 1_554 ?
Ba1B O2 2.573(12) 2_756 ?
Ba1B O4 3.210(6) . ?
Ba1B O5 2.915(11) 1_554 ?
Ba1B O5 2.594(6) 2_756 ?
Ba1B O6 3.223(15) 1_544 ?
Ba1B O6 2.612(11) 2_766 ?
Ba2 Ba2 1.051(3) 2_655 ?
Ba2 Mo1 3.5543(12) 2_655 ?
Ba2 Mo1 3.9193(12) . ?
Ba2 Mo3 3.6459(12) 2_656 ?
Ba2 Mo4 3.8258(13) 1_544 ?
Ba2 O1 2.714(2) 2_655 ?
Ba2 O1 2.507(2) . ?
Ba2 O2 2.590(2) 1_554 ?
Ba2 O3 3.125(2) 1_544 ?
Ba2 O5 2.717(2) 2_656 ?
Ba2 O5 2.547(2) 1_554 ?
Ba2 O6 2.659(2) 1_544 ?
Mo1 Ba2 3.5544(12) 2_655 ?
Mo1 Mo1 2.5796(4) 2_656 ?
Mo1 Mo2 2.5793(3) . ?
Mo1 Mo2 3.1626(3) 1_455 ?
Mo1 Mo2 2.6169(3) 2_656 ?
Mo1 O1 2.0499(17) . ?
Mo1 O1 2.0540(18) 2_656 ?
Mo1 O2 2.0532(18) 2_656 ?
Mo1 O3 2.0536(17) 2_666 ?
Mo1 O7 2.1310(17) 1_455 ?
Mo1 O8 2.0357(18) . ?
Mo2 Mo1 2.6169(3) 2_656 ?
Mo2 Mo1 3.1626(3) 1_655 ?
Mo2 Mo2 3.1714(4) 2_756 ?
Mo2 O1 2.0823(18) . ?
Mo2 O2 2.0914(17) 2_756 ?
Mo2 O2 2.0383(18) . ?
Mo2 O4 2.0188(17) . ?
Mo2 O7 2.1466(19) . ?
Mo2 O8 1.9335(17) . ?
Mo3 Ba2 3.6459(12) 2_656 ?
Mo3 Ba2 3.9209(12) 1_556 ?
Mo3 Mo3 2.5608(4) 2_667 ?
Mo3 Mo4 2.8474(3) 2_667 ?
Mo3 Mo4 2.5484(3) . ?
Mo3 Mo4 3.2004(3) 1_455 ?
Mo3 O3 1.9915(18) . ?
Mo3 O4 2.1295(17) 2_666 ?
Mo3 O5 2.0481(18) 2_667 ?
Mo3 O5 2.0496(18) . ?
Mo3 O6 2.0545(18) 2_667 ?
Mo3 O8 2.0285(17) . ?
Mo4 Ba1A 3.7625(2) 1_556 ?
Mo4 Ba1B 3.742(5) 1_556 ?
Mo4 Ba2 3.8258(13) 1_566 ?
Mo4 Mo3 3.2004(3) 1_655 ?
Mo4 Mo3 2.8474(3) 2_667 ?
Mo4 O3 1.9297(17) . ?
Mo4 O4 2.0753(18) 2_766 ?
Mo4 O5 2.0837(18) . ?
Mo4 O6 2.0439(18) . ?
Mo4 O6 2.1111(18) 2_767 ?
Mo4 O7 1.8976(18) . ?
O1 Ba1B 2.554(6) 2_755 ?
O1 Ba2 2.714(2) 2_655 ?
O1 Mo1 2.0540(18) 2_656 ?
O2 Ba1A 2.8586(18) 1_556 ?
O2 Ba1B 3.192(15) 1_556 ?
O2 Ba1B 2.573(12) 2_756 ?
O2 Ba2 2.590(2) 1_556 ?
O2 Mo1 2.0532(18) 2_656 ?
O2 Mo2 2.0914(17) 2_756 ?
O3 Ba2 3.125(2) 1_566 ?
O3 Mo1 2.0536(17) 2_666 ?
O4 Mo3 2.1295(17) 2_666 ?
O4 Mo4 2.0753(18) 2_766 ?
O5 Ba1A 2.7171(17) 1_556 ?
O5 Ba1B 2.915(11) 1_556 ?
O5 Ba1B 2.594(6) 2_756 ?
O5 Ba2 2.718(2) 2_656 ?
O5 Ba2 2.547(2) 1_556 ?
O5 Mo3 2.0481(18) 2_667 ?
O6 Ba1A 2.8936(18) 1_566 ?
O6 Ba1B 3.223(15) 1_566 ?
O6 Ba1B 2.612(11) 2_766 ?
O6 Ba2 2.659(2) 1_566 ?
O6 Mo3 2.0545(18) 2_667 ?
O6 Mo4 2.1111(18) 2_767 ?
O7 Mo1 2.1310(17) 1_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo2 Ba1A Mo2 180.0 2_755 . ?
Mo2 Ba1A Mo4 87.631(5) . 2_756 ?
Mo2 Ba1A Mo4 87.631(5) 2_755 1_554 ?
Mo2 Ba1A Mo4 92.369(5) . 1_554 ?
Mo2 Ba1A Mo4 92.369(5) 2_755 2_756 ?
Mo4 Ba1A Mo4 180.0 1_554 2_756 ?
O1 Ba1A Mo2 146.05(4) . 2_755 ?
O1 Ba1A Mo2 33.95(4) . . ?
O1 Ba1A Mo2 146.05(4) 2_755 . ?
O1 Ba1A Mo2 33.95(4) 2_755 2_755 ?
O1 Ba1A Mo4 100.68(4) 2_755 2_756 ?
O1 Ba1A Mo4 79.32(4) 2_755 1_554 ?
O1 Ba1A Mo4 79.32(4) . 2_756 ?
O1 Ba1A Mo4 100.68(4) . 1_554 ?
O1 Ba1A O1 180.0 . 2_755 ?
O1 Ba1A O2 116.60(5) . 1_554 ?
O1 Ba1A O2 116.60(5) 2_755 2_756 ?
O1 Ba1A O2 63.40(5) . 2_756 ?
O1 Ba1A O2 63.40(5) 2_755 1_554 ?
O1 Ba1A O5 73.11(5) . 1_554 ?
O1 Ba1A O5 73.11(5) 2_755 2_756 ?
O1 Ba1A O5 106.89(5) . 2_756 ?
O1 Ba1A O5 106.89(5) 2_755 1_554 ?
O1 Ba1A O6 72.99(5) . 1_544 ?
O1 Ba1A O6 72.99(5) 2_755 2_766 ?
O1 Ba1A O6 107.01(5) 2_755 1_544 ?
O1 Ba1A O6 107.01(5) . 2_766 ?
O2 Ba1A Mo2 145.40(3) 2_756 2_755 ?
O2 Ba1A Mo2 145.40(3) 1_554 . ?
O2 Ba1A Mo2 34.60(3) 2_756 . ?
O2 Ba1A Mo2 34.60(3) 1_554 2_755 ?
O2 Ba1A Mo4 106.67(4) 2_756 1_554 ?
O2 Ba1A Mo4 106.67(4) 1_554 2_756 ?
O2 Ba1A Mo4 73.33(4) 2_756 2_756 ?
O2 Ba1A Mo4 73.33(4) 1_554 1_554 ?
O2 Ba1A O2 180.00(2) 2_756 1_554 ?
O2 Ba1A O6 79.94(5) 2_756 2_766 ?
O2 Ba1A O6 79.94(5) 1_554 1_544 ?
O2 Ba1A O6 100.06(5) 2_756 1_544 ?
O2 Ba1A O6 100.06(5) 1_554 2_766 ?
O5 Ba1A Mo2 79.36(4) 1_554 . ?
O5 Ba1A Mo2 100.64(4) 2_756 . ?
O5 Ba1A Mo2 100.64(4) 1_554 2_755 ?
O5 Ba1A Mo2 79.36(4) 2_756 2_755 ?
O5 Ba1A Mo4 32.74(4) 2_756 2_756 ?
O5 Ba1A Mo4 32.74(4) 1_554 1_554 ?
O5 Ba1A Mo4 147.26(4) 2_756 1_554 ?
O5 Ba1A Mo4 147.26(4) 1_554 2_756 ?
O5 Ba1A O2 71.69(5) 2_756 2_756 ?
O5 Ba1A O2 108.31(5) 2_756 1_554 ?
O5 Ba1A O2 71.69(5) 1_554 1_554 ?
O5 Ba1A O2 108.31(5) 1_554 2_756 ?
O5 Ba1A O5 180.0 2_756 1_554 ?
O5 Ba1A O6 118.39(5) 1_554 1_544 ?
O5 Ba1A O6 118.39(5) 2_756 2_766 ?
O5 Ba1A O6 61.61(5) 2_756 1_544 ?
O5 Ba1A O6 61.61(5) 1_554 2_766 ?
O6 Ba1A Mo2 81.80(3) 2_766 . ?
O6 Ba1A Mo2 98.20(3) 2_766 2_755 ?
O6 Ba1A Mo2 98.20(3) 1_544 . ?
O6 Ba1A Mo2 81.80(3) 1_544 2_755 ?
O6 Ba1A Mo4 33.90(3) 1_544 2_756 ?
O6 Ba1A Mo4 146.10(3) 1_544 1_554 ?
O6 Ba1A Mo4 33.90(3) 2_766 1_554 ?
O6 Ba1A Mo4 146.10(3) 2_766 2_756 ?
O6 Ba1A O6 180.00(2) 2_766 1_544 ?
Ba1B Ba1B Mo2 95.5(6) 2_755 . ?
Ba1B Ba1B Mo4 88.7(7) 2_755 1_554 ?
Ba1B Ba1B O1 60.5(6) 2_755 . ?
Ba1B Ba1B O1 100.4(7) 2_755 2_755 ?
Ba1B Ba1B O2 122.2(7) 2_755 2_756 ?
Ba1B Ba1B O2 43.0(5) 2_755 1_554 ?
Ba1B Ba1B O4 100.9(7) 2_755 . ?
Ba1B Ba1B O5 61.3(7) 2_755 1_554 ?
Ba1B Ba1B O5 99.7(7) 2_755 2_756 ?
Ba1B Ba1B O6 121.7(8) 2_755 2_766 ?
Ba1B Ba1B O6 43.6(5) 2_755 1_544 ?
Mo2 Ba1B Mo4 93.96(10) . 1_554 ?
O1 Ba1B Mo2 35.40(6) . . ?
O1 Ba1B Mo2 163.3(7) 2_755 . ?
O1 Ba1B Mo4 81.23(12) 2_755 1_554 ?
O1 Ba1B Mo4 97.3(2) . 1_554 ?
O1 Ba1B O1 160.9(8) 2_755 . ?
O1 Ba1B O2 101.6(6) . 1_554 ?
O1 Ba1B O2 59.8(2) 2_755 1_554 ?
O1 Ba1B O2 133.8(8) 2_755 2_756 ?
O1 Ba1B O4 135.7(4) 2_755 . ?
O1 Ba1B O4 55.26(10) . . ?
O1 Ba1B O5 104.8(2) 2_755 1_554 ?
O1 Ba1B O5 77.33(19) 2_755 2_756 ?
O1 Ba1B O5 67.3(3) . 1_554 ?
O1 Ba1B O6 101.2(3) 2_755 1_544 ?
O1 Ba1B O6 80.0(3) 2_755 2_766 ?
O1 Ba1B O6 65.6(3) . 1_544 ?
O2 Ba1B Mo2 133.6(5) 1_554 . ?
O2 Ba1B Mo2 34.93(7) 2_756 . ?
O2 Ba1B Mo4 70.35(18) 1_554 1_554 ?
O2 Ba1B Mo4 114.1(3) 2_756 1_554 ?
O2 Ba1B O1 64.25(11) 2_756 . ?
O2 Ba1B O2 165.2(6) 2_756 1_554 ?
O2 Ba1B O4 57.27(15) 2_756 . ?
O2 Ba1B O4 119.5(4) 1_554 . ?
O2 Ba1B O5 110.75(15) 2_756 1_554 ?
O2 Ba1B O5 78.4(3) 2_756 2_756 ?
O2 Ba1B O6 70.3(4) 1_554 1_544 ?
O2 Ba1B O6 90.9(5) 2_756 2_766 ?
O2 Ba1B O6 98.41(19) 2_756 1_544 ?
O4 Ba1B Mo2 33.93(6) . . ?
O4 Ba1B Mo4 60.86(8) . 1_554 ?
O4 Ba1B O6 120.8(4) . 1_544 ?
O5 Ba1B Mo2 78.33(14) 1_554 . ?
O5 Ba1B Mo2 105.2(2) 2_756 . ?
O5 Ba1B Mo4 33.66(6) 1_554 1_554 ?
O5 Ba1B Mo4 158.0(3) 2_756 1_554 ?
O5 Ba1B O1 104.5(2) 2_756 . ?
O5 Ba1B O2 64.5(3) 1_554 1_554 ?
O5 Ba1B O2 102.3(3) 2_756 1_554 ?
O5 Ba1B O4 55.03(10) 1_554 . ?
O5 Ba1B O4 135.6(4) 2_756 . ?
O5 Ba1B O5 161.0(8) 2_756 1_554 ?
O5 Ba1B O6 135.6(8) 2_756 2_766 ?
O5 Ba1B O6 58.1(2) 2_756 1_544 ?
O5 Ba1B O6 103.4(6) 1_554 1_544 ?
O6 Ba1B Mo2 87.2(2) 2_766 . ?
O6 Ba1B Mo2 93.9(2) 1_544 . ?
O6 Ba1B Mo4 33.14(10) 2_766 1_554 ?
O6 Ba1B Mo4 132.2(6) 1_544 1_554 ?
O6 Ba1B O1 109.19(16) 2_766 . ?
O6 Ba1B O2 98.4(2) 2_766 1_554 ?
O6 Ba1B O4 55.72(15) 2_766 . ?
O6 Ba1B O5 62.46(12) 2_766 1_554 ?
O6 Ba1B O6 165.3(7) 2_766 1_544 ?
Ba2 Ba2 Mo1 102.54(13) 2_655 2_655 ?
Ba2 Ba2 Mo1 62.28(12) 2_655 . ?
Ba2 Ba2 Mo3 97.32(14) 2_655 2_656 ?
Ba2 Ba2 Mo4 129.21(15) 2_655 1_544 ?
Ba2 Ba2 O1 89.70(13) 2_655 . ?
Ba2 Ba2 O1 67.51(12) 2_655 2_655 ?
Ba2 Ba2 O2 127.53(15) 2_655 1_554 ?
Ba2 Ba2 O3 110.25(14) 2_655 1_544 ?
Ba2 Ba2 O5 69.46(13) 2_655 2_656 ?
Ba2 Ba2 O5 87.80(14) 2_655 1_554 ?
Ba2 Ba2 O6 130.65(15) 2_655 1_544 ?
Mo1 Ba2 Mo1 164.83(4) 2_655 . ?
Mo1 Ba2 Mo3 96.13(3) 2_655 2_656 ?
Mo1 Ba2 Mo4 61.30(2) 2_655 1_544 ?
Mo3 Ba2 Mo1 86.40(2) 2_656 . ?
Mo3 Ba2 Mo4 44.722(15) 2_656 1_544 ?
Mo4 Ba2 Mo1 127.23(3) 1_544 . ?
O1 Ba2 Mo1 27.43(4) . . ?
O1 Ba2 Mo1 129.79(6) 2_655 . ?
O1 Ba2 Mo1 35.03(4) 2_655 2_655 ?
O1 Ba2 Mo1 167.75(7) . 2_655 ?
O1 Ba2 Mo3 81.68(5) . 2_656 ?
O1 Ba2 Mo3 100.55(5) 2_655 2_656 ?
O1 Ba2 Mo4 110.44(6) . 1_544 ?
O1 Ba2 Mo4 85.53(5) 2_655 1_544 ?
O1 Ba2 O1 157.22(6) . 2_655 ?
O1 Ba2 O2 135.40(8) . 1_554 ?
O1 Ba2 O3 55.44(5) 2_655 1_544 ?
O1 Ba2 O3 139.38(7) . 1_544 ?
O1 Ba2 O5 100.14(7) . 2_656 ?
O1 Ba2 O5 79.04(7) . 1_554 ?
O1 Ba2 O5 72.63(6) 2_655 2_656 ?
O1 Ba2 O6 79.95(7) . 1_544 ?
O2 Ba2 Mo1 155.29(6) 1_554 . ?
O2 Ba2 Mo1 34.76(4) 1_554 2_655 ?
O2 Ba2 Mo3 111.97(6) 1_554 2_656 ?
O2 Ba2 Mo4 67.43(5) 1_554 1_544 ?
O2 Ba2 O1 65.05(6) 1_554 2_655 ?
O2 Ba2 O3 56.58(6) 1_554 1_544 ?
O2 Ba2 O5 114.49(7) 1_554 2_656 ?
O2 Ba2 O6 89.51(7) 1_554 1_544 ?
O3 Ba2 Mo1 35.07(3) 1_544 2_655 ?
O3 Ba2 Mo1 146.62(5) 1_544 . ?
O3 Ba2 Mo3 61.48(4) 1_544 2_656 ?
O3 Ba2 Mo4 30.14(3) 1_544 1_544 ?
O5 Ba2 Mo1 90.03(5) 2_656 . ?
O5 Ba2 Mo1 101.59(5) 1_554 2_655 ?
O5 Ba2 Mo1 78.90(5) 1_554 . ?
O5 Ba2 Mo1 84.01(5) 2_656 2_655 ?
O5 Ba2 Mo3 33.75(4) 2_656 2_656 ?
O5 Ba2 Mo3 160.03(6) 1_554 2_656 ?
O5 Ba2 Mo4 61.49(4) 2_656 1_544 ?
O5 Ba2 Mo4 140.37(6) 1_554 1_544 ?
O5 Ba2 O1 99.25(7) 1_554 2_655 ?
O5 Ba2 O2 79.00(6) 1_554 1_554 ?
O5 Ba2 O3 58.50(5) 2_656 1_544 ?
O5 Ba2 O3 134.46(7) 1_554 1_544 ?
O5 Ba2 O5 157.27(6) 1_554 2_656 ?
O5 Ba2 O6 135.63(8) 1_554 1_544 ?
O6 Ba2 Mo1 98.66(5) 1_544 . ?
O6 Ba2 Mo1 91.53(5) 1_544 2_655 ?
O6 Ba2 Mo3 33.64(4) 1_544 2_656 ?
O6 Ba2 Mo4 30.50(4) 1_544 1_544 ?
O6 Ba2 O1 114.42(7) 1_544 2_655 ?
O6 Ba2 O3 60.05(6) 1_544 1_544 ?
O6 Ba2 O5 65.29(6) 1_544 2_656 ?
Ba2 Mo1 Ba2 15.17(4) 2_655 . ?
Mo1 Mo1 Ba2 75.56(2) 2_656 . ?
Mo1 Mo1 Ba2 87.27(2) 2_656 2_655 ?
Mo1 Mo1 Mo2 59.513(9) 2_656 2_656 ?
Mo1 Mo1 Mo2 125.201(12) 2_656 1_455 ?
Mo2 Mo1 Ba2 82.661(19) 2_656 . ?
Mo2 Mo1 Ba2 80.70(2) 1_455 2_655 ?
Mo2 Mo1 Ba2 80.13(2) 2_656 2_655 ?
Mo2 Mo1 Ba2 83.12(2) . . ?
Mo2 Mo1 Ba2 95.38(2) 1_455 . ?
Mo2 Mo1 Ba2 97.26(2) . 2_655 ?
Mo2 Mo1 Mo1 60.964(9) . 2_656 ?
Mo2 Mo1 Mo2 120.477(9) . 2_656 ?
Mo2 Mo1 Mo2 173.148(11) . 1_455 ?
Mo2 Mo1 Mo2 65.773(8) 2_656 1_455 ?
O1 Mo1 Ba2 34.29(5) . . ?
O1 Mo1 Ba2 126.08(5) 2_656 2_655 ?
O1 Mo1 Ba2 120.75(5) 2_656 . ?
O1 Mo1 Ba2 49.46(5) . 2_655 ?
O1 Mo1 Mo1 50.98(5) 2_656 2_656 ?
O1 Mo1 Mo1 51.13(5) . 2_656 ?
O1 Mo1 Mo2 90.33(5) 2_656 . ?
O1 Mo1 Mo2 128.16(5) . 1_455 ?
O1 Mo1 Mo2 51.23(5) 2_656 2_656 ?
O1 Mo1 Mo2 89.37(5) . 2_656 ?
O1 Mo1 Mo2 51.94(5) . . ?
O1 Mo1 Mo2 96.16(5) 2_656 1_455 ?
O1 Mo1 O1 102.11(6) . 2_656 ?
O1 Mo1 O2 88.12(7) . 2_656 ?
O1 Mo1 O3 83.78(7) . 2_666 ?
O1 Mo1 O7 166.32(7) . 1_455 ?
O1 Mo1 O7 89.86(7) 2_656 1_455 ?
O2 Mo1 Ba2 45.98(5) 2_656 2_655 ?
O2 Mo1 Ba2 58.33(5) 2_656 . ?
O2 Mo1 Mo1 96.56(5) 2_656 2_656 ?
O2 Mo1 Mo2 40.71(5) 2_656 1_455 ?
O2 Mo1 Mo2 140.05(5) 2_656 . ?
O2 Mo1 Mo2 49.99(5) 2_656 2_656 ?
O2 Mo1 O1 100.16(7) 2_656 2_656 ?
O2 Mo1 O3 84.04(7) 2_656 2_666 ?
O2 Mo1 O7 83.22(7) 2_656 1_455 ?
O3 Mo1 Ba2 66.43(5) 2_666 . ?
O3 Mo1 Ba2 60.95(6) 2_666 2_655 ?
O3 Mo1 Mo1 134.74(5) 2_666 2_656 ?
O3 Mo1 Mo2 83.16(5) 2_666 1_455 ?
O3 Mo1 Mo2 133.77(5) 2_666 2_656 ?
O3 Mo1 Mo2 90.12(5) 2_666 . ?
O3 Mo1 O1 172.80(7) 2_666 2_656 ?
O3 Mo1 O7 84.80(7) 2_666 1_455 ?
O7 Mo1 Ba2 117.78(5) 1_455 2_655 ?
O7 Mo1 Ba2 132.83(5) 1_455 . ?
O7 Mo1 Mo1 140.37(5) 1_455 2_656 ?
O7 Mo1 Mo2 93.11(5) 1_455 2_656 ?
O7 Mo1 Mo2 135.67(5) 1_455 . ?
O7 Mo1 Mo2 42.51(5) 1_455 1_455 ?
O8 Mo1 Ba2 125.69(5) . . ?
O8 Mo1 Ba2 135.64(5) . 2_655 ?
O8 Mo1 Mo1 94.22(5) . 2_656 ?
O8 Mo1 Mo2 47.77(5) . . ?
O8 Mo1 Mo2 130.33(5) . 1_455 ?
O8 Mo1 Mo2 137.31(5) . 2_656 ?
O8 Mo1 O1 86.13(7) . 2_656 ?
O8 Mo1 O1 99.23(7) . . ?
O8 Mo1 O2 169.19(7) . 2_656 ?
O8 Mo1 O3 88.86(7) . 2_666 ?
O8 Mo1 O7 88.05(7) . 1_455 ?
Mo1 Mo2 Ba1A 81.225(7) 2_656 . ?
Mo1 Mo2 Ba1A 94.540(7) . . ?
Mo1 Mo2 Ba1A 86.915(6) 1_655 . ?
Mo1 Mo2 Ba1B 102.0(3) . . ?
Mo1 Mo2 Ba1B 79.7(3) 1_655 . ?
Mo1 Mo2 Ba1B 86.0(2) 2_656 . ?
Mo1 Mo2 Mo1 59.523(8) . 2_656 ?
Mo1 Mo2 Mo1 173.148(11) . 1_655 ?
Mo1 Mo2 Mo1 114.228(8) 2_656 1_655 ?
Mo1 Mo2 Mo2 124.862(11) . 2_756 ?
Mo1 Mo2 Mo2 48.806(7) 1_655 2_756 ?
Mo1 Mo2 Mo2 65.422(8) 2_656 2_756 ?
Mo2 Mo2 Ba1A 79.656(7) 2_756 . ?
Mo2 Mo2 Ba1B 76.36(16) 2_756 . ?
O1 Mo2 Ba1A 46.01(5) . . ?
O1 Mo2 Ba1B 53.4(3) . . ?
O1 Mo2 Mo1 50.27(5) . 2_656 ?
O1 Mo2 Mo1 128.44(5) . 1_655 ?
O1 Mo2 Mo1 50.82(5) . . ?
O1 Mo2 Mo2 95.31(5) . 2_756 ?
O1 Mo2 O2 88.63(7) . 2_756 ?
O1 Mo2 O7 170.34(7) . . ?
O2 Mo2 Ba1A 111.57(5) . . ?
O2 Mo2 Ba1A 50.91(5) 2_756 . ?
O2 Mo2 Ba1B 44.8(3) 2_756 . ?
O2 Mo2 Ba1B 111.18(10) . . ?
O2 Mo2 Mo1 50.49(5) . 2_656 ?
O2 Mo2 Mo1 89.39(5) 2_756 2_656 ?
O2 Mo2 Mo1 39.82(5) 2_756 1_655 ?
O2 Mo2 Mo1 76.31(5) . 1_655 ?
O2 Mo2 Mo1 96.95(5) . . ?
O2 Mo2 Mo1 138.49(5) 2_756 . ?
O2 Mo2 Mo2 40.45(5) . 2_756 ?
O2 Mo2 Mo2 39.22(5) 2_756 2_756 ?
O2 Mo2 O1 99.71(7) . . ?
O2 Mo2 O2 79.67(7) . 2_756 ?
O2 Mo2 O7 80.70(7) . . ?
O2 Mo2 O7 81.94(7) 2_756 . ?
O4 Mo2 Ba1A 64.25(5) . . ?
O4 Mo2 Ba1B 62.54(10) . . ?
O4 Mo2 Mo1 98.33(5) . . ?
O4 Mo2 Mo1 88.33(5) . 1_655 ?
O4 Mo2 Mo1 137.92(5) . 2_656 ?
O4 Mo2 Mo2 125.69(5) . 2_756 ?
O4 Mo2 O1 87.72(7) . . ?
O4 Mo2 O2 86.90(7) . 2_756 ?
O4 Mo2 O2 164.42(7) . . ?
O4 Mo2 O7 89.70(7) . . ?
O7 Mo2 Ba1A 124.79(5) . . ?
O7 Mo2 Ba1B 117.3(3) . . ?
O7 Mo2 Mo1 131.18(5) . 2_656 ?
O7 Mo2 Mo1 138.83(5) . . ?
O7 Mo2 Mo1 42.13(5) . 1_655 ?
O7 Mo2 Mo2 78.68(5) . 2_756 ?
O8 Mo2 Ba1A 138.83(5) . . ?
O8 Mo2 Ba1B 144.5(2) . . ?
O8 Mo2 Mo1 95.59(6) . 2_656 ?
O8 Mo2 Mo1 130.02(5) . 1_655 ?
O8 Mo2 Mo1 51.22(5) . . ?
O8 Mo2 Mo2 136.19(5) . 2_756 ?
O8 Mo2 O1 101.53(7) . . ?
O8 Mo2 O2 96.51(7) . . ?
O8 Mo2 O2 169.65(7) . 2_756 ?
O8 Mo2 O4 95.37(7) . . ?
O8 Mo2 O7 87.97(7) . . ?
Ba2 Mo3 Ba2 15.42(4) 2_656 1_556 ?
Mo3 Mo3 Ba2 75.527(19) 2_667 1_556 ?
Mo3 Mo3 Ba2 76.96(2) 2_667 2_656 ?
Mo3 Mo3 Mo4 55.924(8) 2_667 2_667 ?
Mo3 Mo3 Mo4 120.731(11) 2_667 1_455 ?
Mo4 Mo3 Ba2 83.168(19) 2_667 1_556 ?
Mo4 Mo3 Ba2 83.21(2) . 1_556 ?
Mo4 Mo3 Ba2 82.37(2) 1_455 2_656 ?
Mo4 Mo3 Ba2 96.14(2) 1_455 1_556 ?
Mo4 Mo3 Ba2 70.99(2) 2_667 2_656 ?
Mo4 Mo3 Ba2 97.89(2) . 2_656 ?
Mo4 Mo3 Mo3 67.740(9) . 2_667 ?
Mo4 Mo3 Mo4 123.663(8) . 2_667 ?
Mo4 Mo3 Mo4 64.866(7) 2_667 1_455 ?
Mo4 Mo3 Mo4 171.134(11) . 1_455 ?
O3 Mo3 Ba2 126.96(5) . 1_556 ?
O3 Mo3 Ba2 142.32(6) . 2_656 ?
O3 Mo3 Mo3 99.32(5) . 2_667 ?
O3 Mo3 Mo4 137.71(5) . 2_667 ?
O3 Mo3 Mo4 48.42(5) . . ?
O3 Mo3 Mo4 128.03(5) . 1_455 ?
O3 Mo3 O4 88.52(7) . 2_666 ?
O3 Mo3 O5 100.87(7) . . ?
O3 Mo3 O5 90.80(7) . 2_667 ?
O3 Mo3 O6 168.33(7) . 2_667 ?
O3 Mo3 O8 89.46(7) . . ?
O4 Mo3 Ba2 120.44(5) 2_666 2_656 ?
O4 Mo3 Ba2 131.80(5) 2_666 1_556 ?
O4 Mo3 Mo3 136.11(5) 2_666 2_667 ?
O4 Mo3 Mo4 89.84(5) 2_666 2_667 ?
O4 Mo3 Mo4 136.66(5) 2_666 . ?
O4 Mo3 Mo4 39.81(5) 2_666 1_455 ?
O5 Mo3 Ba2 113.26(5) 2_667 2_656 ?
O5 Mo3 Ba2 47.44(6) . 2_656 ?
O5 Mo3 Ba2 35.48(6) . 1_556 ?
O5 Mo3 Ba2 120.16(5) 2_667 1_556 ?
O5 Mo3 Mo3 51.30(5) . 2_667 ?
O5 Mo3 Mo3 51.35(5) 2_667 2_667 ?
O5 Mo3 Mo4 52.54(5) . . ?
O5 Mo3 Mo4 90.22(5) 2_667 1_455 ?
O5 Mo3 Mo4 97.76(5) 2_667 . ?
O5 Mo3 Mo4 88.97(5) . 2_667 ?
O5 Mo3 Mo4 129.39(5) . 1_455 ?
O5 Mo3 Mo4 46.96(5) 2_667 2_667 ?
O5 Mo3 O4 167.23(7) . 2_666 ?
O5 Mo3 O4 85.70(7) 2_667 2_666 ?
O5 Mo3 O5 102.65(6) 2_667 . ?
O5 Mo3 O6 89.94(7) . 2_667 ?
O5 Mo3 O6 91.10(7) 2_667 2_667 ?
O6 Mo3 Ba2 45.79(5) 2_667 2_656 ?
O6 Mo3 Ba2 61.12(5) 2_667 1_556 ?
O6 Mo3 Mo3 90.83(5) 2_667 2_667 ?
O6 Mo3 Mo4 45.84(5) 2_667 2_667 ?
O6 Mo3 Mo4 142.47(5) 2_667 . ?
O6 Mo3 Mo4 40.45(5) 2_667 1_455 ?
O6 Mo3 O4 80.15(7) 2_667 2_666 ?
O8 Mo3 Ba2 65.88(5) . 1_556 ?
O8 Mo3 Ba2 70.95(6) . 2_656 ?
O8 Mo3 Mo3 136.91(5) . 2_667 ?
O8 Mo3 Mo4 82.94(5) . 1_455 ?
O8 Mo3 Mo4 132.54(5) . 2_667 ?
O8 Mo3 Mo4 88.76(5) . . ?
O8 Mo3 O4 85.80(7) . 2_666 ?
O8 Mo3 O5 171.49(7) . 2_667 ?
O8 Mo3 O5 85.65(7) . . ?
O8 Mo3 O6 86.98(7) . 2_667 ?
Mo3 Mo4 Ba1A 94.395(7) . 1_556 ?
Mo3 Mo4 Ba1A 76.885(6) 2_667 1_556 ?
Mo3 Mo4 Ba1A 85.289(6) 1_655 1_556 ?
Mo3 Mo4 Ba1B 78.1(3) 1_655 1_556 ?
Mo3 Mo4 Ba1B 78.74(10) 2_667 1_556 ?
Mo3 Mo4 Ba1B 101.2(3) . 1_556 ?
Mo3 Mo4 Ba2 64.289(19) 2_667 1_566 ?
Mo3 Mo4 Ba2 73.64(2) . 1_566 ?
Mo3 Mo4 Ba2 100.93(2) 1_655 1_566 ?
Mo3 Mo4 Mo3 115.133(8) 2_667 1_655 ?
Mo3 Mo4 Mo3 56.337(8) . 2_667 ?
Mo3 Mo4 Mo3 171.134(11) . 1_655 ?
O3 Mo4 Ba1A 141.43(6) . 1_556 ?
O3 Mo4 Ba1B 148.8(3) . 1_556 ?
O3 Mo4 Ba2 54.39(6) . 1_566 ?
O3 Mo4 Mo3 50.53(5) . . ?
O3 Mo4 Mo3 131.99(5) . 1_655 ?
O3 Mo4 Mo3 91.80(5) . 2_667 ?
O3 Mo4 O4 91.07(7) . 2_766 ?
O3 Mo4 O5 101.77(7) . . ?
O3 Mo4 O6 94.61(7) . . ?
O3 Mo4 O6 168.13(8) . 2_767 ?
O4 Mo4 Ba1A 124.34(5) 2_766 1_556 ?
O4 Mo4 Ba1B 117.7(3) 2_766 1_556 ?
O4 Mo4 Ba2 78.16(5) 2_766 1_566 ?
O4 Mo4 Mo3 141.03(5) 2_766 . ?
O4 Mo4 Mo3 41.07(5) 2_766 1_655 ?
O4 Mo4 Mo3 130.70(5) 2_766 2_667 ?
O4 Mo4 O5 166.55(7) 2_766 . ?
O4 Mo4 O6 80.11(7) 2_766 2_767 ?
O5 Mo4 Ba1A 44.86(5) . 1_556 ?
O5 Mo4 Ba1B 50.9(3) . 1_556 ?
O5 Mo4 Ba2 106.04(5) . 1_566 ?
O5 Mo4 Mo3 51.33(5) . . ?
O5 Mo4 Mo3 125.75(5) . 1_655 ?
O5 Mo4 Mo3 45.92(5) . 2_667 ?
O5 Mo4 O6 86.61(7) . 2_767 ?
O6 Mo4 Ba1A 49.87(5) 2_767 1_556 ?
O6 Mo4 Ba1A 102.77(5) . 1_556 ?
O6 Mo4 Ba1B 42.6(3) 2_767 1_556 ?
O6 Mo4 Ba1B 99.62(15) . 1_556 ?
O6 Mo4 Ba2 115.43(5) 2_767 1_566 ?
O6 Mo4 Ba2 41.32(5) . 1_566 ?
O6 Mo4 Mo3 46.15(5) . 2_667 ?
O6 Mo4 Mo3 136.56(5) 2_767 . ?
O6 Mo4 Mo3 91.43(5) . . ?
O6 Mo4 Mo3 88.04(5) 2_767 2_667 ?
O6 Mo4 Mo3 39.16(5) 2_767 1_655 ?
O6 Mo4 Mo3 80.03(5) . 1_655 ?
O6 Mo4 O4 84.57(7) . 2_766 ?
O6 Mo4 O5 90.39(7) . . ?
O6 Mo4 O6 76.77(8) . 2_767 ?
O7 Mo4 Ba1A 67.53(6) . 1_556 ?
O7 Mo4 Ba1B 69.41(12) . 1_556 ?
O7 Mo4 Ba2 151.39(6) . 1_566 ?
O7 Mo4 Mo3 99.87(6) . . ?
O7 Mo4 Mo3 88.21(6) . 1_655 ?
O7 Mo4 Mo3 135.55(6) . 2_667 ?
O7 Mo4 O3 99.58(8) . . ?
O7 Mo4 O4 92.16(8) . 2_766 ?
O7 Mo4 O5 89.63(8) . . ?
O7 Mo4 O6 165.49(7) . . ?
O7 Mo4 O6 88.75(7) . 2_767 ?
Ba1B O1 Ba1B 19.1(8) 2_755 . ?
Ba2 O1 Ba2 22.78(6) . 2_655 ?
Mo1 O1 Ba1A 122.87(8) 2_656 . ?
Mo1 O1 Ba1A 158.49(9) . . ?
Mo1 O1 Ba1B 156.76(17) . . ?
Mo1 O1 Ba1B 156.3(2) . 2_755 ?
Mo1 O1 Ba1B 119.91(18) 2_656 . ?
Mo1 O1 Ba1B 125.20(16) 2_656 2_755 ?
Mo1 O1 Ba2 118.28(8) . . ?
Mo1 O1 Ba2 127.79(9) 2_656 2_655 ?
Mo1 O1 Ba2 95.50(7) . 2_655 ?
Mo1 O1 Ba2 128.88(9) 2_656 . ?
Mo1 O1 Mo1 77.89(6) . 2_656 ?
Mo1 O1 Mo2 77.24(6) . . ?
Mo1 O1 Mo2 78.49(6) 2_656 . ?
Mo2 O1 Ba1A 100.04(7) . . ?
Mo2 O1 Ba1B 110.1(4) . 2_755 ?
Mo2 O1 Ba1B 91.2(3) . . ?
Mo2 O1 Ba2 149.17(9) . . ?
Mo2 O1 Ba2 151.18(9) . 2_655 ?
Ba1B O2 Ba1B 14.8(6) 2_756 1_556 ?
Mo1 O2 Ba1A 147.02(8) 2_656 1_556 ?
Mo1 O2 Ba1B 139.2(4) 2_656 2_756 ?
Mo1 O2 Ba1B 153.1(2) 2_656 1_556 ?
Mo1 O2 Ba2 99.26(7) 2_656 1_556 ?
Mo1 O2 Mo2 99.47(7) 2_656 2_756 ?
Mo2 O2 Ba1A 94.49(6) 2_756 1_556 ?
Mo2 O2 Ba1A 127.11(8) . 1_556 ?
Mo2 O2 Ba1B 123.81(16) . 1_556 ?
Mo2 O2 Ba1B 89.8(2) 2_756 1_556 ?
Mo2 O2 Ba1B 100.3(3) 2_756 2_756 ?
Mo2 O2 Ba1B 130.59(18) . 2_756 ?
Mo2 O2 Ba2 137.01(9) 2_756 1_556 ?
Mo2 O2 Ba2 120.97(8) . 1_556 ?
Mo2 O2 Mo1 79.52(6) . 2_656 ?
Mo2 O2 Mo2 100.33(7) . 2_756 ?
Mo1 O3 Ba2 83.98(6) 2_666 1_566 ?
Mo3 O3 Ba2 98.82(7) . 1_566 ?
Mo3 O3 Mo1 136.45(9) . 2_666 ?
Mo4 O3 Ba2 95.47(7) . 1_566 ?
Mo4 O3 Mo1 142.29(10) . 2_666 ?
Mo4 O3 Mo3 81.05(7) . . ?
Mo2 O4 Ba1B 83.53(10) . . ?
Mo2 O4 Mo3 126.53(9) . 2_666 ?
Mo2 O4 Mo4 133.75(9) . 2_766 ?
Mo3 O4 Ba1B 103.2(3) 2_666 . ?
Mo4 O4 Ba1B 94.0(3) 2_766 . ?
Mo4 O4 Mo3 99.12(7) 2_766 2_666 ?
Ba1B O5 Ba1B 19.0(8) 2_756 1_556 ?
Ba2 O5 Ba2 22.73(6) 1_556 2_656 ?
Mo3 O5 Ba1A 161.08(9) . 1_556 ?
Mo3 O5 Ba1A 121.55(8) 2_667 1_556 ?
Mo3 O5 Ba1B 127.0(2) 2_667 2_756 ?
Mo3 O5 Ba1B 116.1(2) 2_667 1_556 ?
Mo3 O5 Ba1B 154.2(4) . 2_756 ?
Mo3 O5 Ba1B 164.16(12) . 1_556 ?
Mo3 O5 Ba2 126.69(8) 2_667 1_556 ?
Mo3 O5 Ba2 98.81(7) . 2_656 ?
Mo3 O5 Ba2 116.68(8) . 1_556 ?
Mo3 O5 Ba2 111.38(7) 2_667 2_656 ?
Mo3 O5 Mo3 77.35(6) 2_667 . ?
Mo3 O5 Mo4 87.12(7) 2_667 . ?
Mo3 O5 Mo4 76.12(6) . . ?
Mo4 O5 Ba1A 102.40(7) . 1_556 ?
Mo4 O5 Ba1B 110.0(3) . 2_756 ?
Mo4 O5 Ba1B 95.5(3) . 1_556 ?
Mo4 O5 Ba2 159.55(9) . 2_656 ?
Mo4 O5 Ba2 144.86(9) . 1_556 ?
Ba1B O6 Ba1B 14.7(7) 2_766 1_566 ?
Mo3 O6 Ba1A 145.74(8) 2_667 1_566 ?
Mo3 O6 Ba1B 149.15(16) 2_667 1_566 ?
Mo3 O6 Ba1B 140.5(3) 2_667 2_766 ?
Mo3 O6 Ba2 100.57(7) 2_667 1_566 ?
Mo3 O6 Mo4 100.39(7) 2_667 2_767 ?
Mo4 O6 Ba1A 117.03(7) . 1_566 ?
Mo4 O6 Ba1A 96.23(6) 2_767 1_566 ?
Mo4 O6 Ba1B 115.12(15) . 2_766 ?
Mo4 O6 Ba1B 104.3(4) 2_767 2_766 ?
Mo4 O6 Ba1B 89.7(3) 2_767 1_566 ?
Mo4 O6 Ba1B 118.17(11) . 1_566 ?
Mo4 O6 Ba2 108.18(7) . 1_566 ?
Mo4 O6 Ba2 142.54(9) 2_767 1_566 ?
Mo4 O6 Mo3 88.02(7) . 2_667 ?
Mo4 O6 Mo4 103.23(8) . 2_767 ?
Mo1 O7 Mo2 95.35(7) 1_655 . ?
Mo4 O7 Mo1 138.55(10) . 1_655 ?
Mo4 O7 Mo2 126.09(9) . . ?
Mo2 O8 Mo1 81.01(6) . . ?
Mo2 O8 Mo3 137.06(10) . . ?
Mo3 O8 Mo1 141.52(9) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Ba1A Mo4 O7 Mo1 -84.67(14) 1_556 . . 1_655 ?
Ba1A Mo4 O7 Mo2 96.13(11) 1_556 . . . ?
Ba1B Mo4 O7 Mo1 -77.0(3) 1_556 . . 1_655 ?
Ba1B Mo4 O7 Mo2 103.8(3) 1_556 . . . ?
Ba2 Mo4 O7 Mo1 110.77(14) 1_566 . . 1_655 ?
Ba2 Mo4 O7 Mo2 -68.43(18) 1_566 . . . ?
Mo3 Mo4 O7 Mo1 -124.13(12) 2_667 . . 1_655 ?
Mo3 Mo4 O7 Mo1 0.97(14) 1_655 . . 1_655 ?
Mo3 Mo4 O7 Mo1 -175.37(13) . . . 1_655 ?
Mo3 Mo4 O7 Mo2 56.68(14) 2_667 . . . ?
Mo3 Mo4 O7 Mo2 5.43(11) . . . . ?
Mo3 Mo4 O7 Mo2 -178.23(11) 1_655 . . . ?
O3 Mo4 O7 Mo1 133.31(15) . . . 1_655 ?
O3 Mo4 O7 Mo2 -45.89(12) . . . . ?
O4 Mo4 O7 Mo1 41.86(15) 2_766 . . 1_655 ?
O4 Mo4 O7 Mo2 -137.34(11) 2_766 . . . ?
O5 Mo4 O7 Mo1 -124.81(15) . . . 1_655 ?
O5 Mo4 O7 Mo2 55.99(11) . . . . ?
O6 Mo4 O7 Mo1 -34.7(4) . . . 1_655 ?
O6 Mo4 O7 Mo1 -38.20(15) 2_767 . . 1_655 ?
O6 Mo4 O7 Mo2 146.1(2) . . . . ?
O6 Mo4 O7 Mo2 142.60(12) 2_767 . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.773
_oxdiff_exptl_absorpt_empirical_full_min 0.579
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.99752(16)
2 0.00248(16)

_exptl_crystal_recrystallization_method 'Solid state reaction'
_exptl_crystal_preparation       'Magnetic properties'
